# Electronic Supplementary Material (ESI) for Inorganic Chemistry Frontiers.
# This journal is © the Partner Organisations 2023

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_7
_database_code_depnum_ccdc_archive 'CCDC 2181617'
loop_
_audit_author_name
_audit_author_address
'Zhang Ruonan'
;University of Chinese Academy of Sciences
China
;
_audit_update_record             
;
2022-06-24 deposited with the CCDC.	2022-12-05 downloaded from the CCDC.
;
_audit_creation_date             2022-04-19
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'B5 F2 O8 Rb3'
_chemical_formula_sum            'B5 F2 O8 Rb3'
_chemical_formula_weight         476.46
_chemical_absolute_configuration ?
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           4
_space_group_name_H-M_alt        'P 1 21 1'
_space_group_name_Hall           'P 2yb'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z'

_cell_length_a                   6.7342(4)
_cell_length_b                   7.0706(4)
_cell_length_c                   10.0108(6)
_cell_angle_alpha                90
_cell_angle_beta                 93.593(2)
_cell_angle_gamma                90
_cell_volume                     475.73(5)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    5057
_cell_measurement_temperature    273.15
_cell_measurement_theta_max      27.481
_cell_measurement_theta_min      3.530
_shelx_estimated_absorpt_T_max   0.599
_shelx_estimated_absorpt_T_min   0.429
_exptl_absorpt_coefficient_mu    15.427
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_correction_T_min  0.5339
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
'SADABS-2016/2 (Bruker,2016/2) was used for absorption correction. wR2(int) was 0.1025 before and 0.0726 after correction. The Ratio of minimum to maximum transmission is 0.7161. The λ/2 correction factor is Not present.'
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'clear light colourless'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    3.326
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             436
_exptl_crystal_size_max          0.066
_exptl_crystal_size_mid          0.042
_exptl_crystal_size_min          0.037
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0431
_diffrn_reflns_av_unetI/netI     0.0482
_diffrn_reflns_Laue_measured_fraction_full 0.995
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            8119
_diffrn_reflns_point_group_measured_fraction_full 0.987
_diffrn_reflns_point_group_measured_fraction_max 0.988
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.496
_diffrn_reflns_theta_min         2.038
_diffrn_ambient_temperature      273.15
_diffrn_detector_area_resol_mean 5.6
_diffrn_detector_type            'Bruker SMART CCD 6000 area detector'
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device       'three-circle diffractometer'
_diffrn_measurement_device_type  'PHOTON III C28 detector'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.835
_reflns_Friedel_fraction_full    0.977
_reflns_Friedel_fraction_max     0.978
_reflns_number_gt                2010
_reflns_number_total             2158
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences. Completness statistics refer to single and
 composite reflections containing twin component 1 only.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT V8.40B (?, 2016)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT V8.40B (?, 2016)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'olex2.solve 1.3 (Bourhis et al., 2015)'
_refine_diff_density_max         0.603
_refine_diff_density_min         -0.528
_refine_diff_density_rms         0.107
_refine_ls_abs_structure_details 
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.021(12)
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.951
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     164
_refine_ls_number_reflns         2158
_refine_ls_number_restraints     1
_refine_ls_R_factor_all          0.0256
_refine_ls_R_factor_gt           0.0227
_refine_ls_restrained_S_all      0.950
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     'w=1/[σ²(Fo²)] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0427
_refine_ls_wR_factor_ref         0.0435
_refine_special_details          
;
 Refined as a 2-component inversion twin.
;
_olex2_refinement_description    
;
1. Twinned data refinement
 Scales: 0.979(12)
 0.021(12)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Rb2 Rb 0.40893(9) 0.08605(7) 0.84737(6) 0.01794(14) Uani 1 1 d . . . . .
Rb1 Rb 0.29597(10) 0.20821(8) 0.50197(7) 0.02171(15) Uani 1 1 d . . . . .
Rb3 Rb 0.92110(9) 0.91411(8) 0.90505(6) 0.02109(15) Uani 1 1 d . . . . .
F1 F 0.2768(5) 0.5364(4) 0.3400(4) 0.0208(8) Uani 1 1 d . . . . .
F2 F 0.2834(5) 0.7142(5) 0.9553(3) 0.0178(7) Uani 1 1 d . . . . .
O8 O 0.8927(6) 0.5314(5) 0.8241(4) 0.0154(9) Uani 1 1 d . . . . .
O3 O 0.2446(7) 0.7798(5) 0.4978(4) 0.0164(9) Uani 1 1 d . . . . .
O1 O 0.3245(7) 0.7357(5) 0.7243(4) 0.0200(10) Uani 1 1 d . . . . .
O6 O 0.5618(6) 0.5788(6) 0.8729(4) 0.0158(8) Uani 1 1 d . . . . .
O4 O 0.0150(6) 0.7487(5) 0.2945(4) 0.0124(9) Uani 1 1 d . . . . .
O5 O 0.2352(6) 0.4380(5) 0.8230(4) 0.0119(8) Uani 1 1 d . . . . .
O7 O 0.6404(6) 0.3479(5) 0.7108(4) 0.0155(9) Uani 1 1 d . . . . .
O2 O 0.0653(6) 0.5533(5) 0.6196(4) 0.0176(9) Uani 1 1 d . . . . .
B1 B 0.2083(10) 0.6855(8) 0.6114(7) 0.0129(13) Uani 1 1 d . . . . .
B4 B 0.3511(10) 0.6065(9) 0.8377(6) 0.0127(13) Uani 1 1 d . . . . .
B2 B 0.2137(10) 0.7334(8) 0.3562(7) 0.0141(14) Uani 1 1 d . . . . .
B5 B 0.6978(10) 0.4839(8) 0.8020(6) 0.0128(13) Uani 1 1 d . . . . .
B3 B 0.0474(10) 0.4415(8) 0.7443(6) 0.0106(13) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Rb2 Rb3 3.5835(9) 1_445 ?
Rb2 F1 2.935(4) 2_646 ?
Rb2 F2 2.916(3) 2_647 ?
Rb2 F2 2.985(4) 1_545 ?
Rb2 O1 2.809(4) 1_545 ?
Rb2 O6 2.795(4) 2_647 ?
Rb2 O4 3.314(4) 2_546 ?
Rb2 O5 2.754(4) . ?
Rb2 O7 2.827(4) . ?
Rb2 B4 3.455(6) 2_647 ?
Rb2 B4 3.414(6) 1_545 ?
Rb2 B2 3.513(7) 2_646 ?
Rb1 F1 3.418(4) 2_646 ?
Rb1 F1 2.829(3) . ?
Rb1 O3 3.135(5) 2_646 ?
Rb1 O3 3.049(4) 1_545 ?
Rb1 O4 3.025(4) 2_546 ?
Rb1 O7 3.365(4) 2_646 ?
Rb1 O7 3.181(4) . ?
Rb1 O2 3.159(4) . ?
Rb1 O2 2.869(4) 2_546 ?
Rb1 B1 3.516(7) 2_546 ?
Rb1 B5 3.434(6) 2_646 ?
Rb1 B3 3.452(6) . ?
Rb3 F1 2.852(4) 2_656 ?
Rb3 F2 2.837(3) 1_655 ?
Rb3 F2 2.932(4) 2_657 ?
Rb3 O8 2.828(4) . ?
Rb3 O8 3.031(4) 2_757 ?
Rb3 O6 3.388(4) . ?
Rb3 O4 3.143(4) 2_656 ?
Rb3 O5 2.985(4) 2_657 ?
Rb3 B4 3.526(7) 2_657 ?
Rb3 B2 3.530(6) 2_656 ?
Rb3 B3 3.509(6) 2_657 ?
F1 B2 1.468(7) . ?
F2 B4 1.497(7) . ?
O8 B5 1.360(8) . ?
O8 B3 1.494(7) 1_655 ?
O3 B1 1.353(8) . ?
O3 B2 1.457(8) . ?
O1 B1 1.381(8) . ?
O1 B4 1.459(7) . ?
O6 B4 1.454(7) . ?
O6 B5 1.369(7) . ?
O4 B2 1.442(8) . ?
O4 B3 1.472(7) 2_556 ?
O5 B4 1.427(7) . ?
O5 B3 1.447(7) . ?
O7 B2 1.467(8) 2_646 ?
O7 B5 1.365(7) . ?
O2 B1 1.349(7) . ?
O2 B3 1.489(7) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F1 Rb2 Rb3 140.11(7) 2_646 1_445 ?
F1 Rb2 F2 110.97(9) 2_646 1_545 ?
F1 Rb2 O4 113.81(10) 2_646 2_546 ?
F1 Rb2 B4 105.87(14) 2_646 2_647 ?
F1 Rb2 B4 87.06(13) 2_646 1_545 ?
F1 Rb2 B2 24.26(12) 2_646 2_646 ?
F2 Rb2 Rb3 128.01(7) 2_647 1_445 ?
F2 Rb2 Rb3 50.17(6) 1_545 1_445 ?
F2 Rb2 F1 87.71(10) 2_647 2_646 ?
F2 Rb2 F2 103.52(7) 2_647 1_545 ?
F2 Rb2 O4 101.82(9) 1_545 2_546 ?
F2 Rb2 O4 137.64(10) 2_647 2_546 ?
F2 Rb2 B4 80.41(12) 1_545 2_647 ?
F2 Rb2 B4 25.42(12) 2_647 2_647 ?
F2 Rb2 B4 25.96(12) 1_545 1_545 ?
F2 Rb2 B4 113.76(12) 2_647 1_545 ?
F2 Rb2 B2 134.64(12) 1_545 2_646 ?
F2 Rb2 B2 77.98(13) 2_647 2_646 ?
O1 Rb2 Rb3 66.99(10) 1_545 1_445 ?
O1 Rb2 F1 75.44(12) 1_545 2_646 ?
O1 Rb2 F2 47.76(11) 1_545 1_545 ?
O1 Rb2 F2 133.38(11) 1_545 2_647 ?
O1 Rb2 O4 88.44(11) 1_545 2_546 ?
O1 Rb2 O7 117.91(12) 1_545 . ?
O1 Rb2 B4 120.49(13) 1_545 2_647 ?
O1 Rb2 B4 24.76(13) 1_545 1_545 ?
O1 Rb2 B2 98.11(14) 1_545 2_646 ?
O6 Rb2 Rb3 80.80(8) 2_647 1_445 ?
O6 Rb2 F1 129.01(11) 2_647 2_646 ?
O6 Rb2 F2 67.98(11) 2_647 1_545 ?
O6 Rb2 F2 47.51(10) 2_647 2_647 ?
O6 Rb2 O1 115.01(12) 2_647 1_545 ?
O6 Rb2 O4 116.14(11) 2_647 2_546 ?
O6 Rb2 O7 119.33(12) 2_647 . ?
O6 Rb2 B4 24.07(14) 2_647 2_647 ?
O6 Rb2 B4 90.63(14) 2_647 1_545 ?
O6 Rb2 B2 125.32(14) 2_647 2_646 ?
O4 Rb2 Rb3 54.05(7) 2_546 1_445 ?
O4 Rb2 B4 103.81(12) 2_546 1_545 ?
O4 Rb2 B4 135.88(13) 2_546 2_647 ?
O4 Rb2 B2 106.47(13) 2_546 2_646 ?
O5 Rb2 Rb3 86.11(8) . 1_445 ?
O5 Rb2 F1 111.75(11) . 2_646 ?
O5 Rb2 F2 93.39(10) . 2_647 ?
O5 Rb2 F2 134.40(11) . 1_545 ?
O5 Rb2 O1 133.23(11) . 1_545 ?
O5 Rb2 O6 96.21(12) . 2_647 ?
O5 Rb2 O4 45.47(10) . 2_546 ?
O5 Rb2 O7 67.02(12) . . ?
O5 Rb2 B4 147.98(14) . 1_545 ?
O5 Rb2 B4 102.41(14) . 2_647 ?
O5 Rb2 B2 89.96(13) . 2_646 ?
O7 Rb2 Rb3 147.03(9) . 1_445 ?
O7 Rb2 F1 47.77(10) . 2_646 ?
O7 Rb2 F2 158.29(10) . 1_545 ?
O7 Rb2 F2 74.58(11) . 2_647 ?
O7 Rb2 O4 92.98(11) . 2_546 ?
O7 Rb2 B4 134.60(14) . 1_545 ?
O7 Rb2 B4 99.97(14) . 2_647 ?
O7 Rb2 B2 23.74(12) . 2_646 ?
B4 Rb2 Rb3 64.11(11) 1_545 1_445 ?
B4 Rb2 Rb3 104.38(11) 2_647 1_445 ?
B4 Rb2 B4 96.52(15) 1_545 2_647 ?
B4 Rb2 B2 111.32(15) 1_545 2_646 ?
B4 Rb2 B2 101.70(16) 2_647 2_646 ?
B2 Rb2 Rb3 153.87(11) 2_646 1_445 ?
F1 Rb1 F1 124.30(8) . 2_646 ?
F1 Rb1 O3 143.71(10) . 1_545 ?
F1 Rb1 O3 82.96(10) . 2_646 ?
F1 Rb1 O4 107.45(10) . 2_546 ?
F1 Rb1 O7 105.14(10) . 2_646 ?
F1 Rb1 O7 97.30(10) . . ?
F1 Rb1 O2 93.62(11) . 2_546 ?
F1 Rb1 O2 64.81(10) . . ?
F1 Rb1 B1 81.04(13) . 2_546 ?
F1 Rb1 B1 154.29(12) 2_646 2_546 ?
F1 Rb1 B5 100.91(13) 2_646 2_646 ?
F1 Rb1 B5 82.74(12) . 2_646 ?
F1 Rb1 B3 90.23(12) . . ?
F1 Rb1 B3 106.00(12) 2_646 . ?
O3 Rb1 F1 41.85(9) 2_646 2_646 ?
O3 Rb1 F1 75.22(10) 1_545 2_646 ?
O3 Rb1 O3 105.76(11) 1_545 2_646 ?
O3 Rb1 O7 42.10(10) 1_545 2_646 ?
O3 Rb1 O7 43.15(10) 2_646 . ?
O3 Rb1 O7 113.26(11) 1_545 . ?
O3 Rb1 O7 87.59(10) 2_646 2_646 ?
O3 Rb1 O2 135.58(11) 1_545 . ?
O3 Rb1 O2 112.54(10) 2_646 . ?
O3 Rb1 B1 160.19(13) 2_646 2_546 ?
O3 Rb1 B1 81.01(12) 1_545 2_546 ?
O3 Rb1 B5 62.40(13) 1_545 2_646 ?
O3 Rb1 B5 90.48(14) 2_646 2_646 ?
O3 Rb1 B3 115.14(13) 1_545 . ?
O3 Rb1 B3 116.37(13) 2_646 . ?
O4 Rb1 F1 108.65(10) 2_546 2_646 ?
O4 Rb1 O3 135.15(11) 2_546 2_646 ?
O4 Rb1 O3 91.16(11) 2_546 1_545 ?
O4 Rb1 O7 128.22(10) 2_546 2_646 ?
O4 Rb1 O7 92.01(11) 2_546 . ?
O4 Rb1 O2 45.47(9) 2_546 . ?
O4 Rb1 B1 61.73(14) 2_546 2_546 ?
O4 Rb1 B5 133.46(14) 2_546 2_646 ?
O4 Rb1 B3 25.18(12) 2_546 . ?
O7 Rb1 F1 83.52(9) 2_646 2_646 ?
O7 Rb1 F1 41.26(9) . 2_646 ?
O7 Rb1 O7 122.32(8) . 2_646 ?
O7 Rb1 B1 85.40(12) 2_646 2_546 ?
O7 Rb1 B1 151.16(13) . 2_546 ?
O7 Rb1 B5 132.60(14) . 2_646 ?
O7 Rb1 B5 23.13(12) 2_646 2_646 ?
O7 Rb1 B3 153.27(13) 2_646 . ?
O7 Rb1 B3 75.84(13) . . ?
O2 Rb1 F1 121.40(9) . 2_646 ?
O2 Rb1 F1 136.67(10) 2_546 2_646 ?
O2 Rb1 O3 150.77(11) 2_546 2_646 ?
O2 Rb1 O3 61.46(11) 2_546 1_545 ?
O2 Rb1 O4 73.59(11) 2_546 2_546 ?
O2 Rb1 O7 154.90(10) . 2_646 ?
O2 Rb1 O7 65.20(10) 2_546 2_646 ?
O2 Rb1 O7 82.56(10) . . ?
O2 Rb1 O7 164.05(12) 2_546 . ?
O2 Rb1 O2 91.68(7) 2_546 . ?
O2 Rb1 B1 21.47(12) 2_546 2_546 ?
O2 Rb1 B1 70.61(12) . 2_546 ?
O2 Rb1 B5 136.10(13) . 2_646 ?
O2 Rb1 B5 60.32(14) 2_546 2_646 ?
O2 Rb1 B3 92.58(14) 2_546 . ?
O2 Rb1 B3 25.53(12) . . ?
B5 Rb1 B1 76.01(16) 2_646 2_546 ?
B5 Rb1 B3 151.26(16) 2_646 . ?
B3 Rb1 B1 75.38(15) . 2_546 ?
F1 Rb3 Rb2 98.18(7) 2_656 1_665 ?
F1 Rb3 F2 89.00(10) 2_656 2_657 ?
F1 Rb3 O8 146.24(10) 2_656 2_757 ?
F1 Rb3 O6 80.68(9) 2_656 . ?
F1 Rb3 O4 45.60(9) 2_656 2_656 ?
F1 Rb3 O5 126.51(11) 2_656 2_657 ?
F1 Rb3 B4 105.96(13) 2_656 2_657 ?
F1 Rb3 B2 23.68(12) 2_656 2_656 ?
F1 Rb3 B3 147.08(13) 2_656 2_657 ?
F2 Rb3 Rb2 107.10(7) 2_657 1_665 ?
F2 Rb3 Rb2 53.89(7) 1_655 1_665 ?
F2 Rb3 F1 130.84(10) 1_655 2_656 ?
F2 Rb3 F2 134.46(5) 1_655 2_657 ?
F2 Rb3 O8 63.62(10) 2_657 2_757 ?
F2 Rb3 O8 71.02(10) 1_655 2_757 ?
F2 Rb3 O6 105.62(10) 1_655 . ?
F2 Rb3 O6 101.40(9) 2_657 . ?
F2 Rb3 O4 81.11(9) 2_657 2_656 ?
F2 Rb3 O4 109.70(11) 1_655 2_656 ?
F2 Rb3 O5 47.24(9) 2_657 2_657 ?
F2 Rb3 O5 102.42(10) 1_655 2_657 ?
F2 Rb3 B4 24.67(12) 2_657 2_657 ?
F2 Rb3 B4 122.91(12) 1_655 2_657 ?
F2 Rb3 B2 128.92(14) 1_655 2_656 ?
F2 Rb3 B2 77.51(13) 2_657 2_656 ?
F2 Rb3 B3 58.91(12) 2_657 2_657 ?
F2 Rb3 B3 81.54(13) 1_655 2_657 ?
O8 Rb3 Rb2 73.70(8) 2_757 1_665 ?
O8 Rb3 Rb2 108.94(9) . 1_665 ?
O8 Rb3 F1 91.39(10) . 2_656 ?
O8 Rb3 F2 67.42(11) . 1_655 ?
O8 Rb3 F2 143.51(11) . 2_657 ?
O8 Rb3 O8 122.34(11) . 2_757 ?
O8 Rb3 O6 121.96(10) 2_757 . ?
O8 Rb3 O6 42.97(11) . . ?
O8 Rb3 O4 123.20(11) . 2_656 ?
O8 Rb3 O4 107.29(10) 2_757 2_656 ?
O8 Rb3 O5 107.10(11) . 2_657 ?
O8 Rb3 B4 56.35(13) 2_757 2_657 ?
O8 Rb3 B4 123.34(14) . 2_657 ?
O8 Rb3 B2 112.97(13) . 2_656 ?
O8 Rb3 B2 124.08(13) 2_757 2_656 ?
O8 Rb3 B3 109.77(13) . 2_657 ?
O8 Rb3 B3 25.07(13) 2_757 2_657 ?
O6 Rb3 Rb2 151.46(7) . 1_665 ?
O6 Rb3 B4 86.47(12) . 2_657 ?
O6 Rb3 B2 103.19(13) . 2_656 ?
O6 Rb3 B3 97.56(12) . 2_657 ?
O4 Rb3 Rb2 58.59(8) 2_656 1_665 ?
O4 Rb3 O6 126.28(10) 2_656 . ?
O4 Rb3 B4 105.78(13) 2_656 2_657 ?
O4 Rb3 B2 24.07(13) 2_656 2_656 ?
O4 Rb3 B3 126.31(12) 2_656 2_657 ?
O5 Rb3 Rb2 120.47(8) 2_657 1_665 ?
O5 Rb3 O8 47.02(10) 2_657 2_757 ?
O5 Rb3 O6 80.53(10) 2_657 . ?
O5 Rb3 O4 127.40(10) 2_657 2_656 ?
O5 Rb3 B4 23.48(12) 2_657 2_657 ?
O5 Rb3 B2 123.40(13) 2_657 2_656 ?
O5 Rb3 B3 24.07(13) 2_657 2_657 ?
B4 Rb3 Rb2 120.70(11) 2_657 1_665 ?
B4 Rb3 B2 99.96(15) 2_657 2_656 ?
B2 Rb3 Rb2 81.92(12) 2_656 1_665 ?
B3 Rb3 Rb2 98.28(11) 2_657 1_665 ?
B3 Rb3 B4 41.37(15) 2_657 2_657 ?
B3 Rb3 B2 134.61(14) 2_657 2_656 ?
Rb2 F1 Rb1 68.52(8) 2_656 2_656 ?
Rb1 F1 Rb2 117.09(11) . 2_656 ?
Rb1 F1 Rb1 91.11(9) . 2_656 ?
Rb1 F1 Rb3 104.25(11) . 2_646 ?
Rb3 F1 Rb2 78.66(9) 2_646 2_656 ?
Rb3 F1 Rb1 147.18(13) 2_646 2_656 ?
B2 F1 Rb2 100.5(3) . 2_656 ?
B2 F1 Rb1 81.6(3) . 2_656 ?
B2 F1 Rb1 135.9(3) . . ?
B2 F1 Rb3 105.0(3) . 2_646 ?
Rb2 F2 Rb2 108.28(11) 2_657 1_565 ?
Rb2 F2 Rb3 77.70(9) 2_657 2_647 ?
Rb3 F2 Rb2 75.93(8) 1_455 1_565 ?
Rb3 F2 Rb2 164.22(12) 2_647 1_565 ?
Rb3 F2 Rb2 147.30(13) 1_455 2_657 ?
Rb3 F2 Rb3 91.18(10) 1_455 2_647 ?
B4 F2 Rb2 93.2(3) . 1_565 ?
B4 F2 Rb2 97.8(3) . 2_657 ?
B4 F2 Rb3 100.5(3) . 2_647 ?
B4 F2 Rb3 114.5(3) . 1_455 ?
Rb3 O8 Rb3 89.36(11) . 2_747 ?
B5 O8 Rb3 109.3(3) . . ?
B5 O8 Rb3 114.8(3) . 2_747 ?
B5 O8 B3 120.4(5) . 1_655 ?
B3 O8 Rb3 121.6(3) 1_655 . ?
B3 O8 Rb3 95.7(3) 1_655 2_747 ?
Rb1 O3 Rb1 92.82(11) 1_565 2_656 ?
B1 O3 Rb1 120.3(3) . 1_565 ?
B1 O3 Rb1 98.6(3) . 2_656 ?
B1 O3 B2 133.2(5) . . ?
B2 O3 Rb1 104.2(3) . 1_565 ?
B2 O3 Rb1 92.6(3) . 2_656 ?
Rb2 O1 Rb1 101.28(12) 1_565 2_656 ?
Rb2 O1 Rb3 66.89(10) 1_565 1_455 ?
Rb1 O1 Rb3 161.13(12) 2_656 1_455 ?
B1 O1 Rb2 132.4(3) . 1_565 ?
B1 O1 Rb1 81.7(4) . 2_656 ?
B1 O1 Rb3 95.5(4) . 1_455 ?
B1 O1 B4 120.8(5) . . ?
B4 O1 Rb2 101.5(3) . 1_565 ?
B4 O1 Rb1 114.0(4) . 2_656 ?
B4 O1 Rb3 83.5(3) . 1_455 ?
Rb2 O6 Rb2 95.16(11) 2_657 . ?
Rb2 O6 Rb3 83.51(10) 2_657 . ?
Rb3 O6 Rb2 150.94(13) . . ?
B4 O6 Rb2 81.0(3) . . ?
B4 O6 Rb2 104.3(3) . 2_657 ?
B4 O6 Rb3 127.5(3) . . ?
B5 O6 Rb2 71.9(3) . . ?
B5 O6 Rb2 121.4(4) . 2_657 ?
B5 O6 Rb3 84.0(3) . . ?
B5 O6 B4 127.9(5) . . ?
Rb1 O4 Rb2 69.01(8) 2_556 2_556 ?
Rb1 O4 Rb3 119.01(12) 2_556 2_646 ?
Rb3 O4 Rb2 67.36(8) 2_646 2_556 ?
B2 O4 Rb2 155.4(3) . 2_556 ?
B2 O4 Rb1 111.6(3) . 2_556 ?
B2 O4 Rb3 93.2(3) . 2_646 ?
B2 O4 B3 115.1(4) . 2_556 ?
B3 O4 Rb2 89.1(3) 2_556 2_556 ?
B3 O4 Rb1 93.8(3) 2_556 2_556 ?
B3 O4 Rb3 125.3(3) 2_556 2_646 ?
Rb2 O5 Rb3 92.31(11) . 2_647 ?
B4 O5 Rb2 121.3(3) . . ?
B4 O5 Rb3 100.1(3) . 2_647 ?
B4 O5 B3 119.7(4) . . ?
B3 O5 Rb2 114.6(3) . . ?
B3 O5 Rb3 98.7(3) . 2_647 ?
Rb2 O7 Rb1 153.84(15) . 2_656 ?
Rb2 O7 Rb1 73.32(9) . . ?
Rb1 O7 Rb1 86.30(10) . 2_656 ?
B2 O7 Rb2 105.4(3) 2_646 . ?
B2 O7 Rb1 90.6(3) 2_646 . ?
B2 O7 Rb1 90.7(3) 2_646 2_656 ?
B5 O7 Rb2 106.2(3) . . ?
B5 O7 Rb1 145.3(4) . . ?
B5 O7 Rb1 81.2(3) . 2_656 ?
B5 O7 B2 121.7(5) . 2_646 ?
Rb1 O2 Rb1 124.09(13) 2_556 . ?
B1 O2 Rb1 98.2(4) . . ?
B1 O2 Rb1 107.4(3) . 2_556 ?
B1 O2 B3 121.0(5) . . ?
B3 O2 Rb1 116.6(3) . 2_556 ?
B3 O2 Rb1 88.3(3) . . ?
Rb1 B1 Rb1 96.77(16) 2_556 . ?
Rb1 B1 Rb1 76.89(13) 2_656 . ?
Rb1 B1 Rb1 142.5(2) 2_556 2_656 ?
O3 B1 Rb1 85.9(3) . 2_556 ?
O3 B1 Rb1 59.5(3) . 2_656 ?
O3 B1 Rb1 99.5(4) . . ?
O3 B1 O1 116.0(5) . . ?
O1 B1 Rb1 137.6(4) . 2_556 ?
O1 B1 Rb1 113.2(4) . . ?
O1 B1 Rb1 75.9(3) . 2_656 ?
O2 B1 Rb1 137.0(4) . 2_656 ?
O2 B1 Rb1 60.1(3) . . ?
O2 B1 Rb1 51.1(3) . 2_556 ?
O2 B1 O3 124.1(6) . . ?
O2 B1 O1 119.9(5) . . ?
Rb2 B4 Rb2 167.2(2) 1_565 . ?
Rb2 B4 Rb2 83.80(13) 2_657 . ?
Rb2 B4 Rb2 88.26(15) 1_565 2_657 ?
Rb2 B4 Rb3 115.22(18) 1_565 2_647 ?
Rb2 B4 Rb3 60.16(10) 1_565 1_455 ?
Rb2 B4 Rb3 131.22(19) . 1_455 ?
Rb2 B4 Rb3 63.40(11) 2_657 2_647 ?
Rb2 B4 Rb3 100.61(16) 2_657 1_455 ?
Rb3 B4 Rb2 69.88(12) 2_647 . ?
Rb3 B4 Rb3 69.31(12) 2_647 1_455 ?
F2 B4 Rb2 60.8(3) . 1_565 ?
F2 B4 Rb2 56.7(2) . 2_657 ?
F2 B4 Rb2 121.5(3) . . ?
F2 B4 Rb3 44.0(2) . 1_455 ?
F2 B4 Rb3 54.8(3) . 2_647 ?
O1 B4 Rb2 53.7(3) . 1_565 ?
O1 B4 Rb2 139.8(4) . 2_657 ?
O1 B4 Rb2 130.6(4) . . ?
O1 B4 Rb3 73.5(3) . 1_455 ?
O1 B4 Rb3 140.0(4) . 2_647 ?
O1 B4 F2 105.3(5) . . ?
O6 B4 Rb2 51.6(2) . 2_657 ?
O6 B4 Rb2 76.1(3) . . ?
O6 B4 Rb2 91.1(3) . 1_565 ?
O6 B4 Rb3 108.4(3) . 2_647 ?
O6 B4 Rb3 142.6(4) . 1_455 ?
O6 B4 F2 102.6(4) . . ?
O6 B4 O1 110.1(5) . . ?
O5 B4 Rb2 39.5(2) . . ?
O5 B4 Rb2 153.3(4) . 1_565 ?
O5 B4 Rb2 106.3(3) . 2_657 ?
O5 B4 Rb3 94.6(3) . 1_455 ?
O5 B4 Rb3 56.4(3) . 2_647 ?
O5 B4 F2 108.3(5) . . ?
O5 B4 O1 113.8(5) . . ?
O5 B4 O6 115.6(5) . . ?
Rb2 B2 Rb1 154.94(19) 2_656 2_556 ?
Rb2 B2 Rb1 113.78(18) 2_656 1_565 ?
Rb2 B2 Rb1 61.58(12) 2_656 2_656 ?
Rb2 B2 Rb3 62.78(11) 2_656 2_646 ?
Rb1 B2 Rb1 133.9(2) 2_656 2_556 ?
Rb1 B2 Rb1 76.84(13) 2_656 1_565 ?
Rb1 B2 Rb1 90.66(15) 1_565 2_556 ?
Rb1 B2 Rb3 117.27(19) 2_656 2_646 ?
Rb3 B2 Rb1 92.89(15) 2_646 2_556 ?
Rb3 B2 Rb1 154.2(2) 2_646 1_565 ?
F1 B2 Rb2 55.2(3) . 2_656 ?
F1 B2 Rb1 105.7(3) . 2_556 ?
F1 B2 Rb1 74.1(3) . 2_656 ?
F1 B2 Rb1 150.4(4) . 1_565 ?
F1 B2 Rb3 51.3(2) . 2_646 ?
O3 B2 Rb2 124.5(4) . 2_656 ?
O3 B2 Rb1 53.2(2) . 1_565 ?
O3 B2 Rb1 74.0(3) . 2_556 ?
O3 B2 Rb1 63.0(3) . 2_656 ?
O3 B2 Rb3 151.5(4) . 2_646 ?
O3 B2 F1 107.2(5) . . ?
O3 B2 O7 105.2(5) . 2_656 ?
O4 B2 Rb2 117.3(4) . 2_656 ?
O4 B2 Rb1 102.3(3) . 1_565 ?
O4 B2 Rb1 177.9(4) . 2_656 ?
O4 B2 Rb1 47.8(3) . 2_556 ?
O4 B2 Rb3 62.7(3) . 2_646 ?
O4 B2 F1 106.9(4) . . ?
O4 B2 O3 118.1(5) . . ?
O4 B2 O7 113.1(5) . 2_656 ?
O7 B2 Rb2 50.9(3) 2_656 2_656 ?
O7 B2 Rb1 65.8(3) 2_656 1_565 ?
O7 B2 Rb1 64.8(3) 2_656 2_656 ?
O7 B2 Rb1 147.5(4) 2_656 2_556 ?
O7 B2 Rb3 99.4(3) 2_656 2_646 ?
O7 B2 F1 105.4(5) 2_656 . ?
Rb1 B5 Rb2 139.90(18) 2_656 2_657 ?
O8 B5 Rb2 92.3(3) . 2_657 ?
O8 B5 Rb1 88.0(3) . 2_656 ?
O8 B5 O6 117.7(5) . . ?
O8 B5 O7 120.8(5) . . ?
O6 B5 Rb2 40.2(3) . 2_657 ?
O6 B5 Rb1 106.2(4) . 2_656 ?
O7 B5 Rb2 135.1(4) . 2_657 ?
O7 B5 Rb1 75.6(3) . 2_656 ?
O7 B5 O6 121.5(6) . . ?
Rb2 B3 Rb1 155.47(19) . 2_556 ?
Rb1 B3 Rb2 61.28(10) . . ?
Rb1 B3 Rb1 94.81(15) . 2_556 ?
Rb1 B3 Rb3 132.46(19) . 2_647 ?
Rb3 B3 Rb2 71.20(12) 2_647 . ?
Rb3 B3 Rb1 132.59(18) 2_647 2_556 ?
O8 B3 Rb2 128.7(3) 1_455 . ?
O8 B3 Rb1 73.6(3) 1_455 2_556 ?
O8 B3 Rb1 164.6(4) 1_455 . ?
O8 B3 Rb3 59.3(3) 1_455 2_647 ?
O4 B3 Rb2 66.8(3) 2_546 . ?
O4 B3 Rb1 97.9(3) 2_546 2_556 ?
O4 B3 Rb1 61.0(3) 2_546 . ?
O4 B3 Rb3 102.2(3) 2_546 2_647 ?
O4 B3 O8 109.8(5) 2_546 1_455 ?
O4 B3 O2 107.9(4) 2_546 . ?
O5 B3 Rb2 44.0(2) . . ?
O5 B3 Rb1 147.4(3) . 2_556 ?
O5 B3 Rb1 85.9(3) . . ?
O5 B3 Rb3 57.2(3) . 2_647 ?
O5 B3 O8 109.3(5) . 1_455 ?
O5 B3 O4 110.7(4) . 2_546 ?
O5 B3 O2 110.6(5) . . ?
O2 B3 Rb2 121.4(4) . . ?
O2 B3 Rb1 42.8(3) . 2_556 ?
O2 B3 Rb1 66.2(3) . . ?
O2 B3 Rb3 149.9(4) . 2_647 ?
O2 B3 O8 108.6(4) . 1_455 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Rb2 F1 B2 Rb1 161.82(14) 2_656 . . 2_556 ?
Rb2 F1 B2 Rb1 -76.8(8) 2_656 . . 1_565 ?
Rb2 F1 B2 Rb1 -66.16(12) 2_656 . . 2_656 ?
Rb2 F1 B2 Rb3 80.96(16) 2_656 . . 2_646 ?
Rb2 F1 B2 O3 -120.5(4) 2_656 . . . ?
Rb2 F1 B2 O4 111.9(4) 2_656 . . . ?
Rb2 F1 B2 O7 -8.8(4) 2_656 . . 2_656 ?
Rb2 F2 B4 Rb2 -108.96(14) 2_657 . . 1_565 ?
Rb2 F2 B4 Rb2 108.96(14) 1_565 . . 2_657 ?
Rb2 F2 B4 Rb2 165.4(3) 1_565 . . . ?
Rb2 F2 B4 Rb2 56.4(3) 2_657 . . . ?
Rb2 F2 B4 Rb3 -76.01(18) 1_565 . . 1_455 ?
Rb2 F2 B4 Rb3 175.0(3) 2_657 . . 1_455 ?
Rb2 F2 B4 Rb3 -172.17(17) 1_565 . . 2_647 ?
Rb2 F2 B4 Rb3 78.86(13) 2_657 . . 2_647 ?
Rb2 F2 B4 O1 -140.1(4) 2_657 . . . ?
Rb2 F2 B4 O1 -31.1(4) 1_565 . . . ?
Rb2 F2 B4 O6 84.1(4) 1_565 . . . ?
Rb2 F2 B4 O6 -24.9(4) 2_657 . . . ?
Rb2 F2 B4 O5 97.8(4) 2_657 . . . ?
Rb2 F2 B4 O5 -153.2(4) 1_565 . . . ?
Rb2 O1 B1 Rb1 97.7(4) 1_565 . . 2_656 ?
Rb2 O1 B1 Rb1 -62.1(7) 1_565 . . 2_556 ?
Rb2 O1 B1 Rb1 166.5(2) 1_565 . . . ?
Rb2 O1 B1 O3 52.5(8) 1_565 . . . ?
Rb2 O1 B1 O2 -125.8(5) 1_565 . . . ?
Rb2 O1 B4 Rb2 -164.6(3) 1_565 . . . ?
Rb2 O1 B4 Rb2 -22.2(7) 1_565 . . 2_657 ?
Rb2 O1 B4 Rb3 87.0(5) 1_565 . . 2_647 ?
Rb2 O1 B4 Rb3 64.77(15) 1_565 . . 1_455 ?
Rb2 O1 B4 F2 34.0(4) 1_565 . . . ?
Rb2 O1 B4 O6 -75.9(4) 1_565 . . . ?
Rb2 O1 B4 O5 152.5(4) 1_565 . . . ?
Rb2 O6 B4 Rb2 180.00(16) . . . 1_565 ?
Rb2 O6 B4 Rb2 93.08(16) . . . 2_657 ?
Rb2 O6 B4 Rb2 86.92(18) 2_657 . . 1_565 ?
Rb2 O6 B4 Rb2 -93.08(16) 2_657 . . . ?
Rb2 O6 B4 Rb3 62.91(19) . . . 2_647 ?
Rb2 O6 B4 Rb3 142.6(5) . . . 1_455 ?
Rb2 O6 B4 Rb3 -30.2(3) 2_657 . . 2_647 ?
Rb2 O6 B4 Rb3 49.5(6) 2_657 . . 1_455 ?
Rb2 O6 B4 F2 119.7(4) . . . . ?
Rb2 O6 B4 F2 26.6(4) 2_657 . . . ?
Rb2 O6 B4 O1 138.4(4) 2_657 . . . ?
Rb2 O6 B4 O1 -128.5(4) . . . . ?
Rb2 O6 B4 O5 2.0(4) . . . . ?
Rb2 O6 B4 O5 -91.0(5) 2_657 . . . ?
Rb2 O6 B5 Rb2 -84.9(3) . . . 2_657 ?
Rb2 O6 B5 Rb1 122.1(3) . . . 2_656 ?
Rb2 O6 B5 Rb1 -152.93(18) 2_657 . . 2_656 ?
Rb2 O6 B5 O8 -56.5(6) 2_657 . . . ?
Rb2 O6 B5 O8 -141.4(5) . . . . ?
Rb2 O6 B5 O7 124.3(5) 2_657 . . . ?
Rb2 O6 B5 O7 39.3(5) . . . . ?
Rb2 O4 B2 Rb2 68.8(9) 2_556 . . 2_656 ?
Rb2 O4 B2 Rb1 -86.4(8) 2_556 . . 2_556 ?
Rb2 O4 B2 Rb1 -165.9(7) 2_556 . . 1_565 ?
Rb2 O4 B2 Rb3 36.6(8) 2_556 . . 2_646 ?
Rb2 O4 B2 F1 9.7(11) 2_556 . . . ?
Rb2 O4 B2 O3 -111.2(8) 2_556 . . . ?
Rb2 O4 B2 O7 125.3(7) 2_556 . . 2_656 ?
Rb2 O5 B4 Rb2 -57.9(4) . . . 2_657 ?
Rb2 O5 B4 Rb2 -178.6(6) . . . 1_565 ?
Rb2 O5 B4 Rb3 -99.0(3) . . . 2_647 ?
Rb2 O5 B4 Rb3 -160.36(19) . . . 1_455 ?
Rb2 O5 B4 F2 -117.5(4) . . . . ?
Rb2 O5 B4 O1 125.7(4) . . . . ?
Rb2 O5 B4 O6 -3.1(6) . . . . ?
Rb2 O5 B3 Rb1 -51.7(2) . . . . ?
Rb2 O5 B3 Rb1 -144.3(5) . . . 2_556 ?
Rb2 O5 B3 Rb3 96.6(2) . . . 2_647 ?
Rb2 O5 B3 O8 126.1(3) . . . 1_455 ?
Rb2 O5 B3 O4 5.1(6) . . . 2_546 ?
Rb2 O5 B3 O2 -114.4(4) . . . . ?
Rb2 O7 B5 Rb2 -4.8(6) . . . 2_657 ?
Rb2 O7 B5 Rb1 -154.30(18) . . . 2_656 ?
Rb2 O7 B5 O8 126.9(5) . . . . ?
Rb2 O7 B5 O6 -53.9(6) . . . . ?
Rb1 F1 B2 Rb2 66.16(12) 2_656 . . 2_656 ?
Rb1 F1 B2 Rb2 149.0(5) . . . 2_656 ?
Rb1 F1 B2 Rb1 -49.2(5) . . . 2_556 ?
Rb1 F1 B2 Rb1 82.8(4) . . . 2_656 ?
Rb1 F1 B2 Rb1 72.2(9) . . . 1_565 ?
Rb1 F1 B2 Rb1 -132.0(2) 2_656 . . 2_556 ?
Rb1 F1 B2 Rb1 -10.6(7) 2_656 . . 1_565 ?
Rb1 F1 B2 Rb3 147.12(16) 2_656 . . 2_646 ?
Rb1 F1 B2 Rb3 -130.1(5) . . . 2_646 ?
Rb1 F1 B2 O3 28.5(7) . . . . ?
Rb1 F1 B2 O3 -54.3(4) 2_656 . . . ?
Rb1 F1 B2 O4 -99.1(5) . . . . ?
Rb1 F1 B2 O4 178.1(4) 2_656 . . . ?
Rb1 F1 B2 O7 57.4(4) 2_656 . . 2_656 ?
Rb1 F1 B2 O7 140.2(4) . . . 2_656 ?
Rb1 O3 B1 Rb1 -167.01(18) 1_565 . . . ?
Rb1 O3 B1 Rb1 -98.4(3) 1_565 . . 2_656 ?
Rb1 O3 B1 Rb1 -164.80(11) 2_656 . . 2_556 ?
Rb1 O3 B1 Rb1 -68.6(2) 2_656 . . . ?
Rb1 O3 B1 Rb1 96.8(3) 1_565 . . 2_556 ?
Rb1 O3 B1 O1 -45.3(7) 1_565 . . . ?
Rb1 O3 B1 O1 53.1(5) 2_656 . . . ?
Rb1 O3 B1 O2 -128.8(6) 2_656 . . . ?
Rb1 O3 B1 O2 132.8(5) 1_565 . . . ?
Rb1 O3 B2 Rb2 2.0(3) 2_656 . . 2_656 ?
Rb1 O3 B2 Rb2 95.6(3) 1_565 . . 2_656 ?
Rb1 O3 B2 Rb1 -103.27(16) 1_565 . . 2_556 ?
Rb1 O3 B2 Rb1 163.17(12) 2_656 . . 2_556 ?
Rb1 O3 B2 Rb1 93.57(17) 1_565 . . 2_656 ?
Rb1 O3 B2 Rb1 -93.57(17) 2_656 . . 1_565 ?
Rb1 O3 B2 Rb3 97.9(8) 2_656 . . 2_646 ?
Rb1 O3 B2 Rb3 -168.5(7) 1_565 . . 2_646 ?
Rb1 O3 B2 F1 61.2(4) 2_656 . . . ?
Rb1 O3 B2 F1 154.8(4) 1_565 . . . ?
Rb1 O3 B2 O4 -178.0(4) 2_656 . . . ?
Rb1 O3 B2 O4 -84.4(5) 1_565 . . . ?
Rb1 O3 B2 O7 42.9(5) 1_565 . . 2_656 ?
Rb1 O3 B2 O7 -50.6(4) 2_656 . . 2_656 ?
Rb1 O1 B1 Rb1 -159.9(5) 2_656 . . 2_556 ?
Rb1 O1 B1 Rb1 68.8(3) 2_656 . . . ?
Rb1 O1 B1 O3 -45.3(5) 2_656 . . . ?
Rb1 O1 B1 O2 136.5(6) 2_656 . . . ?
Rb1 O1 B4 Rb2 85.8(6) 2_656 . . 2_657 ?
Rb1 O1 B4 Rb2 108.0(3) 2_656 . . 1_565 ?
Rb1 O1 B4 Rb2 -56.6(5) 2_656 . . . ?
Rb1 O1 B4 Rb3 -165.0(4) 2_656 . . 2_647 ?
Rb1 O1 B4 Rb3 172.8(2) 2_656 . . 1_455 ?
Rb1 O1 B4 F2 142.0(3) 2_656 . . . ?
Rb1 O1 B4 O6 32.1(5) 2_656 . . . ?
Rb1 O1 B4 O5 -99.5(5) 2_656 . . . ?
Rb1 O4 B2 Rb2 155.22(17) 2_556 . . 2_656 ?
Rb1 O4 B2 Rb1 -79.5(2) 2_556 . . 1_565 ?
Rb1 O4 B2 Rb3 123.0(2) 2_556 . . 2_646 ?
Rb1 O4 B2 F1 96.1(4) 2_556 . . . ?
Rb1 O4 B2 O3 -24.8(6) 2_556 . . . ?
Rb1 O4 B2 O7 -148.2(4) 2_556 . . 2_656 ?
Rb1 O7 B5 Rb2 79.2(7) . . . 2_657 ?
Rb1 O7 B5 Rb2 149.5(5) 2_656 . . 2_657 ?
Rb1 O7 B5 Rb1 -70.3(6) . . . 2_656 ?
Rb1 O7 B5 O8 -78.8(5) 2_656 . . . ?
Rb1 O7 B5 O8 -149.0(4) . . . . ?
Rb1 O7 B5 O6 30.1(10) . . . . ?
Rb1 O7 B5 O6 100.4(5) 2_656 . . . ?
Rb1 O2 B1 Rb1 -129.0(4) 2_556 . . 2_656 ?
Rb1 O2 B1 Rb1 -129.7(2) 2_556 . . . ?
Rb1 O2 B1 Rb1 129.7(2) . . . 2_556 ?
Rb1 O2 B1 Rb1 0.7(6) . . . 2_656 ?
Rb1 O2 B1 O3 -48.9(7) 2_556 . . . ?
Rb1 O2 B1 O3 80.8(6) . . . . ?
Rb1 O2 B1 O1 129.2(5) 2_556 . . . ?
Rb1 O2 B1 O1 -101.1(5) . . . . ?
Rb1 O2 B3 Rb2 155.42(19) 2_556 . . . ?
Rb1 O2 B3 Rb2 27.7(3) . . . . ?
Rb1 O2 B3 Rb1 127.7(2) 2_556 . . . ?
Rb1 O2 B3 Rb1 -127.7(2) . . . 2_556 ?
Rb1 O2 B3 Rb3 -97.0(7) 2_556 . . 2_647 ?
Rb1 O2 B3 Rb3 135.2(7) . . . 2_647 ?
Rb1 O2 B3 O8 -36.7(5) 2_556 . . 1_455 ?
Rb1 O2 B3 O8 -164.5(4) . . . 1_455 ?
Rb1 O2 B3 O4 82.2(4) 2_556 . . 2_546 ?
Rb1 O2 B3 O4 -45.6(4) . . . 2_546 ?
Rb1 O2 B3 O5 75.6(4) . . . . ?
Rb1 O2 B3 O5 -156.7(3) 2_556 . . . ?
Rb3 F1 B2 Rb2 -80.96(16) 2_646 . . 2_656 ?
Rb3 F1 B2 Rb1 -147.12(16) 2_646 . . 2_656 ?
Rb3 F1 B2 Rb1 -157.7(6) 2_646 . . 1_565 ?
Rb3 F1 B2 Rb1 80.9(2) 2_646 . . 2_556 ?
Rb3 F1 B2 O3 158.6(4) 2_646 . . . ?
Rb3 F1 B2 O4 31.0(5) 2_646 . . . ?
Rb3 F1 B2 O7 -89.7(4) 2_646 . . 2_656 ?
Rb3 F2 B4 Rb2 -118.6(3) 1_455 . . . ?
Rb3 F2 B4 Rb2 -78.86(13) 2_647 . . 2_657 ?
Rb3 F2 B4 Rb2 -175.0(3) 1_455 . . 2_657 ?
Rb3 F2 B4 Rb2 -22.4(3) 2_647 . . . ?
Rb3 F2 B4 Rb2 172.17(17) 2_647 . . 1_565 ?
Rb3 F2 B4 Rb2 76.01(18) 1_455 . . 1_565 ?
Rb3 F2 B4 Rb3 96.2(2) 2_647 . . 1_455 ?
Rb3 F2 B4 Rb3 -96.2(2) 1_455 . . 2_647 ?
Rb3 F2 B4 O1 44.9(5) 1_455 . . . ?
Rb3 F2 B4 O1 141.1(4) 2_647 . . . ?
Rb3 F2 B4 O6 160.1(3) 1_455 . . . ?
Rb3 F2 B4 O6 -103.7(4) 2_647 . . . ?
Rb3 F2 B4 O5 19.0(4) 2_647 . . . ?
Rb3 F2 B4 O5 -77.2(4) 1_455 . . . ?
Rb3 O8 B5 Rb2 37.6(3) 2_747 . . 2_657 ?
Rb3 O8 B5 Rb2 -60.9(2) . . . 2_657 ?
Rb3 O8 B5 Rb1 177.49(16) 2_747 . . 2_656 ?
Rb3 O8 B5 Rb1 78.9(2) . . . 2_656 ?
Rb3 O8 B5 O6 70.2(6) 2_747 . . . ?
Rb3 O8 B5 O6 -28.3(6) . . . . ?
Rb3 O8 B5 O7 -110.6(5) 2_747 . . . ?
Rb3 O8 B5 O7 150.9(4) . . . . ?
Rb3 O1 B1 Rb1 1.3(5) 1_455 . . 2_556 ?
Rb3 O1 B1 Rb1 -130.0(2) 1_455 . . . ?
Rb3 O1 B1 Rb1 161.20(12) 1_455 . . 2_656 ?
Rb3 O1 B1 O3 115.9(5) 1_455 . . . ?
Rb3 O1 B1 O2 -62.3(6) 1_455 . . . ?
Rb3 O1 B4 Rb2 -64.77(15) 1_455 . . 1_565 ?
Rb3 O1 B4 Rb2 -87.0(5) 1_455 . . 2_657 ?
Rb3 O1 B4 Rb2 130.6(4) 1_455 . . . ?
Rb3 O1 B4 Rb3 22.3(5) 1_455 . . 2_647 ?
Rb3 O1 B4 F2 -30.8(4) 1_455 . . . ?
Rb3 O1 B4 O6 -140.7(4) 1_455 . . . ?
Rb3 O1 B4 O5 87.8(5) 1_455 . . . ?
Rb3 O6 B4 Rb2 -92.8(3) . . . 2_657 ?
Rb3 O6 B4 Rb2 -5.9(4) . . . 1_565 ?
Rb3 O6 B4 Rb2 174.1(3) . . . . ?
Rb3 O6 B4 Rb3 -123.0(3) . . . 2_647 ?
Rb3 O6 B4 Rb3 -43.3(7) . . . 1_455 ?
Rb3 O6 B4 F2 -66.2(5) . . . . ?
Rb3 O6 B4 O1 45.6(6) . . . . ?
Rb3 O6 B4 O5 176.2(3) . . . . ?
Rb3 O6 B5 Rb2 78.6(3) . . . 2_657 ?
Rb3 O6 B5 Rb1 -74.3(2) . . . 2_656 ?
Rb3 O6 B5 O8 22.1(5) . . . . ?
Rb3 O6 B5 O7 -157.1(5) . . . . ?
Rb3 O4 B2 Rb2 32.2(3) 2_646 . . 2_656 ?
Rb3 O4 B2 Rb1 -123.0(2) 2_646 . . 2_556 ?
Rb3 O4 B2 Rb1 157.54(16) 2_646 . . 1_565 ?
Rb3 O4 B2 F1 -26.8(4) 2_646 . . . ?
Rb3 O4 B2 O3 -147.7(4) 2_646 . . . ?
Rb3 O4 B2 O7 88.8(4) 2_646 . . 2_656 ?
Rb3 O5 B4 Rb2 99.0(3) 2_647 . . . ?
Rb3 O5 B4 Rb2 -79.6(8) 2_647 . . 1_565 ?
Rb3 O5 B4 Rb2 41.1(3) 2_647 . . 2_657 ?
Rb3 O5 B4 Rb3 -61.40(18) 2_647 . . 1_455 ?
Rb3 O5 B4 F2 -18.6(4) 2_647 . . . ?
Rb3 O5 B4 O1 -135.4(4) 2_647 . . . ?
Rb3 O5 B4 O6 95.8(5) 2_647 . . . ?
Rb3 O5 B3 Rb2 -96.6(2) 2_647 . . . ?
Rb3 O5 B3 Rb1 -148.32(12) 2_647 . . . ?
Rb3 O5 B3 Rb1 119.2(6) 2_647 . . 2_556 ?
Rb3 O5 B3 O8 29.5(4) 2_647 . . 1_455 ?
Rb3 O5 B3 O4 -91.5(4) 2_647 . . 2_546 ?
Rb3 O5 B3 O2 149.0(4) 2_647 . . . ?
B1 O3 B2 Rb2 -102.3(7) . . . 2_656 ?
B1 O3 B2 Rb1 162.1(7) . . . 1_565 ?
B1 O3 B2 Rb1 58.8(6) . . . 2_556 ?
B1 O3 B2 Rb1 -104.4(6) . . . 2_656 ?
B1 O3 B2 Rb3 -6.4(13) . . . 2_646 ?
B1 O3 B2 F1 -43.1(9) . . . . ?
B1 O3 B2 O4 77.6(8) . . . . ?
B1 O3 B2 O7 -155.0(6) . . . 2_656 ?
B1 O1 B4 Rb2 -179.5(5) . . . 2_657 ?
B1 O1 B4 Rb2 -157.3(6) . . . 1_565 ?
B1 O1 B4 Rb2 38.1(8) . . . . ?
B1 O1 B4 Rb3 -70.3(8) . . . 2_647 ?
B1 O1 B4 Rb3 -92.5(5) . . . 1_455 ?
B1 O1 B4 F2 -123.3(6) . . . . ?
B1 O1 B4 O6 126.8(6) . . . . ?
B1 O1 B4 O5 -4.8(8) . . . . ?
B1 O2 B3 Rb2 -70.9(6) . . . . ?
B1 O2 B3 Rb1 -98.6(5) . . . . ?
B1 O2 B3 Rb1 133.7(6) . . . 2_556 ?
B1 O2 B3 Rb3 36.7(10) . . . 2_647 ?
B1 O2 B3 O8 97.0(6) . . . 1_455 ?
B1 O2 B3 O4 -144.1(5) . . . 2_546 ?
B1 O2 B3 O5 -23.0(7) . . . . ?
B4 O1 B1 Rb1 -113.1(5) . . . 2_656 ?
B4 O1 B1 Rb1 -44.3(7) . . . . ?
B4 O1 B1 Rb1 87.1(7) . . . 2_556 ?
B4 O1 B1 O3 -158.4(5) . . . . ?
B4 O1 B1 O2 23.4(9) . . . . ?
B4 O6 B5 Rb2 -147.4(7) . . . 2_657 ?
B4 O6 B5 Rb1 59.7(6) . . . 2_656 ?
B4 O6 B5 O8 156.1(5) . . . . ?
B4 O6 B5 O7 -23.2(9) . . . . ?
B4 O5 B3 Rb2 156.5(6) . . . . ?
B4 O5 B3 Rb1 104.8(4) . . . . ?
B4 O5 B3 Rb1 12.3(10) . . . 2_556 ?
B4 O5 B3 Rb3 -106.9(5) . . . 2_647 ?
B4 O5 B3 O8 -77.4(6) . . . 1_455 ?
B4 O5 B3 O4 161.6(5) . . . 2_546 ?
B4 O5 B3 O2 42.1(7) . . . . ?
B2 O3 B1 Rb1 -63.0(6) . . . 2_556 ?
B2 O3 B1 Rb1 101.8(6) . . . 2_656 ?
B2 O3 B1 Rb1 33.2(7) . . . . ?
B2 O3 B1 O1 154.9(6) . . . . ?
B2 O3 B1 O2 -26.9(10) . . . . ?
B2 O7 B5 Rb2 -125.1(5) 2_646 . . 2_657 ?
B2 O7 B5 Rb1 85.4(5) 2_646 . . 2_656 ?
B2 O7 B5 O8 6.7(8) 2_646 . . . ?
B2 O7 B5 O6 -174.1(5) 2_646 . . . ?
B5 O6 B4 Rb2 58.6(5) . . . . ?
B5 O6 B4 Rb2 -121.4(5) . . . 1_565 ?
B5 O6 B4 Rb2 151.7(6) . . . 2_657 ?
B5 O6 B4 Rb3 121.5(5) . . . 2_647 ?
B5 O6 B4 Rb3 -158.8(5) . . . 1_455 ?
B5 O6 B4 F2 178.3(5) . . . . ?
B5 O6 B4 O1 -69.9(7) . . . . ?
B5 O6 B4 O5 60.7(7) . . . . ?
B3 O8 B5 Rb2 151.0(4) 1_655 . . 2_657 ?
B3 O8 B5 Rb1 -69.1(4) 1_655 . . 2_656 ?
B3 O8 B5 O6 -176.4(5) 1_655 . . . ?
B3 O8 B5 O7 2.8(8) 1_655 . . . ?
B3 O4 B2 Rb2 -99.4(5) 2_556 . . 2_656 ?
B3 O4 B2 Rb1 25.9(5) 2_556 . . 1_565 ?
B3 O4 B2 Rb1 105.4(5) 2_556 . . 2_556 ?
B3 O4 B2 Rb3 -131.7(4) 2_556 . . 2_646 ?
B3 O4 B2 F1 -158.5(4) 2_556 . . . ?
B3 O4 B2 O3 80.6(6) 2_556 . . . ?
B3 O4 B2 O7 -42.9(7) 2_556 . . 2_656 ?
B3 O5 B4 Rb2 -154.9(6) . . . . ?
B3 O5 B4 Rb2 147.2(4) . . . 2_657 ?
B3 O5 B4 Rb2 26.5(11) . . . 1_565 ?
B3 O5 B4 Rb3 44.7(5) . . . 1_455 ?
B3 O5 B4 Rb3 106.1(5) . . . 2_647 ?
B3 O5 B4 F2 87.5(6) . . . . ?
B3 O5 B4 O1 -29.2(8) . . . . ?
B3 O5 B4 O6 -158.0(5) . . . . ?
B3 O2 B1 Rb1 -137.3(6) . . . 2_556 ?
B3 O2 B1 Rb1 93.6(7) . . . 2_656 ?
B3 O2 B1 Rb1 93.0(5) . . . . ?
B3 O2 B1 O3 173.7(5) . . . . ?
B3 O2 B1 O1 -8.2(8) . . . . ?

_olex2_submission_special_instructions 'No special instructions were received'
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
1 0.979(12)
2 0.021(12)

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_mo_zrn20210203001_0m
_database_code_depnum_ccdc_archive 'CCDC 2181618'
loop_
_audit_author_name
_audit_author_address
'Zhang Ruonan'
;University of Chinese Academy of Sciences
China
;
_audit_update_record             
;
2022-06-24 deposited with the CCDC.	2022-12-05 downloaded from the CCDC.
;
_audit_creation_date             2022-04-19
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2016/6
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'B5 F2 K0.6 O8 Rb2.4'
_chemical_formula_sum            'B5 F2 K0.60 O8 Rb2.40'
_chemical_formula_weight         448.64
_chemical_absolute_configuration ?
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           4
_space_group_name_H-M_alt        'P 1 21 1'
_space_group_name_Hall           'P 2yb'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z'

_cell_length_a                   6.7132(6)
_cell_length_b                   6.9794(7)
_cell_length_c                   9.9534(11)
_cell_angle_alpha                90
_cell_angle_beta                 94.099(4)
_cell_angle_gamma                90
_cell_volume                     465.16(8)
_cell_formula_units_Z            2
_cell_measurement_reflns_used    1424
_cell_measurement_temperature    273(2)
_cell_measurement_theta_max      26.02
_cell_measurement_theta_min      3.79
_shelx_estimated_absorpt_T_max   0.773
_shelx_estimated_absorpt_T_min   0.542
_exptl_absorpt_coefficient_mu    12.927
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_correction_T_min  0.5865
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
'SADABS-2016/2 (Bruker,2016/2) was used for absorption correction. wR2(int) was 0.1021 before and 0.0788 after correction. The Ratio of minimum to maximum transmission is 0.7866. The λ/2 correction factor is Not present.'
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'clear light colourless'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    3.203
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             414
_exptl_crystal_size_max          0.054
_exptl_crystal_size_mid          0.035
_exptl_crystal_size_min          0.021
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0691
_diffrn_reflns_av_unetI/netI     0.0840
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.992
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            5857
_diffrn_reflns_point_group_measured_fraction_full 0.993
_diffrn_reflns_point_group_measured_fraction_max 0.985
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.562
_diffrn_reflns_theta_min         2.051
_diffrn_ambient_temperature      273.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measurement_device_type  'PHOTON III C28 detector'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.835
_reflns_Friedel_fraction_full    0.987
_reflns_Friedel_fraction_max     0.977
_reflns_number_gt                1875
_reflns_number_total             2127
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT V8.40B (?, 2016)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT V8.40B (?, 2016)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'XL (Sheldrick, 2008)'
_computing_structure_solution    'XT (Sheldrick, 2015)'
_refine_diff_density_max         0.613
_refine_diff_density_min         -0.628
_refine_diff_density_rms         0.152
_refine_ls_abs_structure_details 
;
 Flack x determined using 720 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   0.023(15)
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.954
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     163
_refine_ls_number_reflns         2127
_refine_ls_number_restraints     1
_refine_ls_R_factor_all          0.0466
_refine_ls_R_factor_gt           0.0396
_refine_ls_restrained_S_all      0.954
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     'w=1/[σ²(Fo²)] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0706
_refine_ls_wR_factor_ref         0.0744
_refine_special_details          ?
_olex2_refinement_description    
;
1. Shared sites
{K3, Rb3}
2. Uiso/Uaniso restraints and constraints
Uanis(K3) = Uanis(Rb3)
3. Others
 Fixed Sof: K3(0.6) Rb3(0.4)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
K3 K 0.5881(2) 0.0851(2) 0.15182(15) 0.0208(3) Uani 0.6 1 d . . P . .
Rb1 Rb 0.70430(15) 0.20277(13) 0.49526(11) 0.0212(2) Uani 1 1 d . . . . .
Rb2 Rb 0.07453(15) 0.91502(15) 0.09584(10) 0.0225(3) Uani 1 1 d . . . . .
Rb3 Rb 0.5881(2) 0.0851(2) 0.15182(15) 0.0208(3) Uani 0.4 1 d . . P . .
B1 B 0.3037(15) 0.4798(15) 0.1971(11) 0.012(2) Uani 1 1 d . . . . .
B2 B 0.6518(16) 0.6040(15) 0.1594(10) 0.012(2) Uani 1 1 d . . . . .
B3 B 0.9524(14) 0.4371(15) 0.2562(10) 0.009(2) Uani 1 1 d . . . . .
B4 B 0.7914(14) 0.6855(16) 0.3881(11) 0.012(2) Uani 1 1 d . . . . .
B5 B 0.7847(16) 0.7267(16) 0.6448(11) 0.014(2) Uani 1 1 d . . . . .
O1 O 0.1063(9) 0.5324(9) 0.1771(7) 0.0148(15) Uani 1 1 d . . . . .
O2 O 0.3603(9) 0.3439(10) 0.2863(7) 0.0161(15) Uani 1 1 d . . . . .
O3 O 0.4366(9) 0.5783(10) 0.1237(6) 0.0154(14) Uani 1 1 d . . . . .
O4 O 0.7634(9) 0.4336(9) 0.1753(6) 0.0126(13) Uani 1 1 d . . . . .
O5 O 0.6782(10) 0.7383(9) 0.2726(7) 0.0173(16) Uani 1 1 d . . . . .
O6 O 0.9317(10) 0.5479(9) 0.3808(6) 0.0172(16) Uani 1 1 d . . . . .
O7 O 0.7498(10) 0.7754(9) 0.5019(6) 0.0132(14) Uani 1 1 d . . . . .
O8 O 0.9837(9) 0.7419(9) 0.7073(7) 0.0121(15) Uani 1 1 d . . . . .
F1 F 0.7151(7) 0.7119(8) 0.0399(5) 0.0174(12) Uani 1 1 d . . . . .
F2 F 0.7194(8) 0.5293(8) 0.6614(6) 0.0194(13) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
K3 B1 3.400(10) . ?
K3 B2 3.385(11) 1_545 ?
K3 B2 3.391(10) 2_645 ?
K3 B5 3.473(11) 2_646 ?
K3 O2 2.773(7) . ?
K3 O3 2.736(7) 2_645 ?
K3 O4 2.705(7) . ?
K3 O5 2.750(6) 1_545 ?
K3 O8 3.294(6) 2_746 ?
K3 F1 2.831(5) 2_645 ?
K3 F1 2.981(6) 1_545 ?
K3 F2 2.901(6) 2_646 ?
Rb1 B1 3.438(10) 2_646 ?
Rb1 B4 3.502(10) 2_746 ?
Rb1 B5 3.477(11) 2_646 ?
Rb1 O2 3.365(7) 2_646 ?
Rb1 O2 3.153(6) . ?
Rb1 O6 2.869(6) 2_746 ?
Rb1 O6 3.111(7) . ?
Rb1 O7 2.999(6) 1_545 ?
Rb1 O7 3.093(7) 2_646 ?
Rb1 O8 3.022(7) 2_746 ?
Rb1 F2 2.814(5) . ?
Rb1 F2 3.370(6) 2_646 ?
Rb2 B2 3.498(11) 2_655 ?
Rb2 B3 3.499(10) 2_655 ?
Rb2 B5 3.455(11) 2_656 ?
Rb2 O1 2.794(6) . ?
Rb2 O1 3.009(7) 2 ?
Rb2 O3 3.378(7) . ?
Rb2 O4 2.984(6) 2_655 ?
Rb2 O5 3.516(8) 1_455 ?
Rb2 O8 3.051(6) 2_656 ?
Rb2 F1 2.896(6) 2_655 ?
Rb2 F1 2.820(5) 1_455 ?
Rb2 F2 2.812(6) 2_656 ?
B1 O1 1.376(12) . ?
B1 O2 1.336(12) . ?
B1 O3 1.377(12) . ?
B2 O3 1.474(12) . ?
B2 O4 1.408(12) . ?
B2 O5 1.466(12) . ?
B2 F1 1.496(12) . ?
B3 O1 1.499(12) 1_655 ?
B3 O4 1.454(11) . ?
B3 O6 1.476(12) . ?
B3 O8 1.466(12) 2_746 ?
B4 O5 1.382(12) . ?
B4 O6 1.351(12) . ?
B4 O7 1.342(13) . ?
B5 O2 1.477(12) 2_656 ?
B5 O7 1.465(12) . ?
B5 O8 1.437(12) . ?
B5 F2 1.458(12) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
B1 K3 B5 42.0(2) . 2_646 ?
B2 K3 B1 81.7(3) 2_645 . ?
B2 K3 B1 150.7(3) 1_545 . ?
B2 K3 B2 96.3(3) 1_545 2_645 ?
B2 K3 B5 101.9(3) 2_645 2_646 ?
B2 K3 B5 111.4(3) 1_545 2_646 ?
O2 K3 B1 22.1(2) . . ?
O2 K3 B2 135.1(2) . 1_545 ?
O2 K3 B2 100.0(2) . 2_645 ?
O2 K3 B5 24.2(2) . 2_646 ?
O2 K3 O8 94.16(18) . 2_746 ?
O2 K3 F1 158.75(18) . 1_545 ?
O2 K3 F1 74.15(18) . 2_645 ?
O2 K3 F2 48.37(17) . 2_646 ?
O3 K3 B1 98.8(2) 2_645 . ?
O3 K3 B2 90.2(2) 2_645 1_545 ?
O3 K3 B2 25.0(2) 2_645 2_645 ?
O3 K3 B5 126.5(2) 2_645 2_646 ?
O3 K3 O2 120.0(2) 2_645 . ?
O3 K3 O5 114.7(2) 2_645 1_545 ?
O3 K3 O8 114.90(18) 2_645 2_746 ?
O3 K3 F1 66.97(18) 2_645 1_545 ?
O3 K3 F1 48.75(16) 2_645 2_645 ?
O3 K3 F2 130.16(18) 2_645 2_646 ?
O4 K3 B1 60.3(2) . . ?
O4 K3 B2 146.8(2) . 1_545 ?
O4 K3 B2 102.7(2) . 2_645 ?
O4 K3 B5 91.2(2) . 2_646 ?
O4 K3 O2 67.90(19) . . ?
O4 K3 O3 95.6(2) . 2_645 ?
O4 K3 O5 132.29(19) . 1_545 ?
O4 K3 O8 45.84(16) . 2_746 ?
O4 K3 F1 93.70(18) . 2_645 ?
O4 K3 F1 133.14(17) . 1_545 ?
O4 K3 F2 112.97(18) . 2_646 ?
O5 K3 B1 139.7(2) 1_545 . ?
O5 K3 B2 25.0(2) 1_545 1_545 ?
O5 K3 B2 120.6(2) 1_545 2_645 ?
O5 K3 B5 98.1(2) 1_545 2_646 ?
O5 K3 O2 118.3(2) 1_545 . ?
O5 K3 O8 87.05(18) 1_545 2_746 ?
O5 K3 F1 48.29(17) 1_545 1_545 ?
O5 K3 F1 134.01(18) 1_545 2_645 ?
O5 K3 F2 75.31(19) 1_545 2_646 ?
O8 K3 B1 98.9(2) 2_746 . ?
O8 K3 B2 102.4(2) 2_746 1_545 ?
O8 K3 B2 136.0(2) 2_746 2_645 ?
O8 K3 B5 107.5(2) 2_746 2_646 ?
F1 K3 B1 56.8(2) 2_645 . ?
F1 K3 B1 159.3(2) 1_545 . ?
F1 K3 B2 25.9(2) 2_645 2_645 ?
F1 K3 B2 79.8(2) 1_545 2_645 ?
F1 K3 B2 114.1(2) 2_645 1_545 ?
F1 K3 B2 26.2(2) 1_545 1_545 ?
F1 K3 B5 134.7(2) 1_545 2_646 ?
F1 K3 B5 77.9(2) 2_645 2_646 ?
F1 K3 O8 138.30(17) 2_645 2_746 ?
F1 K3 O8 100.68(15) 1_545 2_746 ?
F1 K3 F1 103.43(12) 2_645 1_545 ?
F1 K3 F2 87.90(16) 2_645 2_646 ?
F2 K3 B1 65.9(2) 2_646 . ?
F2 K3 B2 106.1(2) 2_646 2_645 ?
F2 K3 B2 87.0(2) 2_646 1_545 ?
F2 K3 B5 24.4(2) 2_646 2_646 ?
F2 K3 O8 114.27(17) 2_646 2_746 ?
F2 K3 F1 110.97(15) 2_646 1_545 ?
B1 Rb1 B4 76.4(3) 2_646 2_746 ?
B1 Rb1 B5 107.7(2) 2_646 2_646 ?
B5 Rb1 B4 175.7(3) 2_646 2_746 ?
O2 Rb1 B1 132.2(2) . 2_646 ?
O2 Rb1 B1 22.6(2) 2_646 2_646 ?
O2 Rb1 B4 151.0(2) . 2_746 ?
O2 Rb1 B4 85.8(2) 2_646 2_746 ?
O2 Rb1 B5 25.1(2) . 2_646 ?
O2 Rb1 B5 97.6(2) 2_646 2_646 ?
O2 Rb1 O2 122.44(13) . 2_646 ?
O2 Rb1 F2 41.64(15) . 2_646 ?
O2 Rb1 F2 83.57(14) 2_646 2_646 ?
O6 Rb1 B1 60.9(2) 2_746 2_646 ?
O6 Rb1 B1 135.7(2) . 2_646 ?
O6 Rb1 B4 70.1(2) . 2_746 ?
O6 Rb1 B4 21.7(2) 2_746 2_746 ?
O6 Rb1 B5 160.2(2) 2_746 2_646 ?
O6 Rb1 B5 106.8(2) . 2_646 ?
O6 Rb1 O2 82.64(16) . . ?
O6 Rb1 O2 164.26(18) 2_746 . ?
O6 Rb1 O2 65.60(17) 2_746 2_646 ?
O6 Rb1 O2 154.46(16) . 2_646 ?
O6 Rb1 O6 91.38(11) 2_746 . ?
O6 Rb1 O7 62.19(18) 2_746 1_545 ?
O6 Rb1 O7 150.20(18) 2_746 2_646 ?
O6 Rb1 O8 73.22(18) 2_746 2_746 ?
O6 Rb1 F2 136.77(16) 2_746 2_646 ?
O6 Rb1 F2 121.91(15) . 2_646 ?
O7 Rb1 B1 62.5(2) 1_545 2_646 ?
O7 Rb1 B1 89.3(2) 2_646 2_646 ?
O7 Rb1 B4 158.9(2) 2_646 2_746 ?
O7 Rb1 B4 82.2(2) 1_545 2_746 ?
O7 Rb1 B5 24.9(2) 2_646 2_646 ?
O7 Rb1 B5 98.5(2) 1_545 2_646 ?
O7 Rb1 O2 86.76(16) 2_646 2_646 ?
O7 Rb1 O2 42.52(16) 1_545 2_646 ?
O7 Rb1 O2 113.20(18) 1_545 . ?
O7 Rb1 O2 43.84(16) 2_646 . ?
O7 Rb1 O6 136.58(18) 1_545 . ?
O7 Rb1 O6 112.71(16) 2_646 . ?
O7 Rb1 O7 105.18(17) 1_545 2_646 ?
O7 Rb1 O8 91.74(17) 1_545 2_746 ?
O7 Rb1 F2 74.59(16) 1_545 2_646 ?
O7 Rb1 F2 42.53(15) 2_646 2_646 ?
O8 Rb1 B1 133.7(2) 2_746 2_646 ?
O8 Rb1 B4 61.6(2) 2_746 2_746 ?
O8 Rb1 B5 114.1(2) 2_746 2_646 ?
O8 Rb1 O2 128.75(17) 2_746 2_646 ?
O8 Rb1 O2 92.38(17) 2_746 . ?
O8 Rb1 O6 45.89(16) 2_746 . ?
O8 Rb1 O7 136.22(17) 2_746 2_646 ?
O8 Rb1 F2 109.03(16) 2_746 2_646 ?
F2 Rb1 B1 100.5(2) 2_646 2_646 ?
F2 Rb1 B1 81.1(2) . 2_646 ?
F2 Rb1 B4 154.8(2) 2_646 2_746 ?
F2 Rb1 B4 80.8(2) . 2_746 ?
F2 Rb1 B5 101.0(2) . 2_646 ?
F2 Rb1 B5 24.5(2) 2_646 2_646 ?
F2 Rb1 O2 97.39(17) . . ?
F2 Rb1 O2 102.95(16) . 2_646 ?
F2 Rb1 O6 65.81(17) . . ?
F2 Rb1 O6 93.35(18) . 2_746 ?
F2 Rb1 O7 81.72(16) . 2_646 ?
F2 Rb1 O7 142.50(17) . 1_545 ?
F2 Rb1 O8 108.75(17) . 2_746 ?
F2 Rb1 F2 123.84(12) . 2_646 ?
B2 Rb2 B3 41.3(2) 2_655 2_655 ?
B2 Rb2 O5 162.0(2) 2_655 1_455 ?
B3 Rb2 O5 121.99(19) 2_655 1_455 ?
B5 Rb2 B2 100.1(2) 2_656 2_655 ?
B5 Rb2 B3 135.4(2) 2_656 2_655 ?
B5 Rb2 O5 91.3(2) 2_656 1_455 ?
O1 Rb2 B2 122.5(2) . 2_655 ?
O1 Rb2 B2 56.0(2) 2 2_655 ?
O1 Rb2 B3 25.2(2) 2 2_655 ?
O1 Rb2 B3 109.2(2) . 2_655 ?
O1 Rb2 B5 112.0(2) . 2_656 ?
O1 Rb2 B5 125.1(2) 2 2_656 ?
O1 Rb2 O1 122.63(18) . 2 ?
O1 Rb2 O3 43.25(17) . . ?
O1 Rb2 O3 120.34(17) 2 . ?
O1 Rb2 O4 106.14(19) . 2_655 ?
O1 Rb2 O5 106.04(16) 2 1_455 ?
O1 Rb2 O5 64.20(16) . 1_455 ?
O1 Rb2 O8 108.32(17) 2 2_656 ?
O1 Rb2 O8 122.65(18) . 2_656 ?
O1 Rb2 F1 142.11(17) . 2_655 ?
O1 Rb2 F1 67.87(18) . 1_455 ?
O1 Rb2 F2 89.98(17) . 2_656 ?
O3 Rb2 B2 84.8(2) . 2_655 ?
O3 Rb2 B3 95.6(2) . 2_655 ?
O3 Rb2 B5 102.7(2) . 2_656 ?
O3 Rb2 O5 106.29(15) . 1_455 ?
O4 Rb2 B2 23.4(2) 2_655 2_655 ?
O4 Rb2 B3 24.28(19) 2_655 2_655 ?
O4 Rb2 B5 123.4(2) 2_655 2_656 ?
O4 Rb2 O1 47.26(17) 2_655 2 ?
O4 Rb2 O3 78.33(16) 2_655 . ?
O4 Rb2 O5 143.66(16) 2_655 1_455 ?
O4 Rb2 O8 128.33(18) 2_655 2_656 ?
O8 Rb2 B2 106.4(2) 2_656 2_655 ?
O8 Rb2 B3 127.6(2) 2_656 2_655 ?
O8 Rb2 B5 24.5(2) 2_656 2_656 ?
O8 Rb2 O3 126.30(16) 2_656 . ?
O8 Rb2 O5 78.74(16) 2_656 1_455 ?
F1 Rb2 B2 24.8(2) 2_655 2_655 ?
F1 Rb2 B2 122.2(2) 1_455 2_655 ?
F1 Rb2 B3 80.92(19) 1_455 2_655 ?
F1 Rb2 B3 59.6(2) 2_655 2_655 ?
F1 Rb2 B5 77.4(2) 2_655 2_656 ?
F1 Rb2 B5 130.4(2) 1_455 2_656 ?
F1 Rb2 O1 64.07(15) 2_655 2 ?
F1 Rb2 O1 70.98(16) 1_455 2 ?
F1 Rb2 O3 105.48(17) 1_455 . ?
F1 Rb2 O3 99.45(15) 2_655 . ?
F1 Rb2 O4 101.85(16) 1_455 2_655 ?
F1 Rb2 O4 47.59(17) 2_655 2_655 ?
F1 Rb2 O5 153.65(14) 2_655 1_455 ?
F1 Rb2 O5 41.84(15) 1_455 1_455 ?
F1 Rb2 O8 110.84(17) 1_455 2_656 ?
F1 Rb2 O8 81.58(16) 2_655 2_656 ?
F1 Rb2 F1 134.96(9) 1_455 2_655 ?
F2 Rb2 B2 105.4(2) 2_656 2_655 ?
F2 Rb2 B3 146.6(2) 2_656 2_655 ?
F2 Rb2 B5 24.2(2) 2_656 2_656 ?
F2 Rb2 O1 147.17(17) 2_656 2 ?
F2 Rb2 O3 79.62(15) 2_656 . ?
F2 Rb2 O4 125.16(17) 2_656 2_655 ?
F2 Rb2 O5 90.75(15) 2_656 1_455 ?
F2 Rb2 O8 46.68(15) 2_656 2_656 ?
F2 Rb2 F1 132.36(16) 2_656 1_455 ?
F2 Rb2 F1 88.36(15) 2_656 2_655 ?
K3 B1 Rb1 122.0(3) . 2_656 ?
K3 B1 Rb2 98.9(2) . 2_545 ?
K3 B1 Rb2 154.1(3) . . ?
Rb1 B1 Rb2 80.2(2) 2_656 . ?
Rb1 B1 Rb2 133.9(3) 2_656 2_545 ?
Rb2 B1 Rb2 67.91(19) . 2_545 ?
O1 B1 K3 137.8(6) . . ?
O1 B1 Rb1 86.1(5) . 2_656 ?
O1 B1 Rb2 48.0(4) . . ?
O1 B1 Rb2 47.8(4) . 2_545 ?
O1 B1 O3 116.3(9) . . ?
O2 B1 K3 51.5(5) . . ?
O2 B1 Rb1 75.6(5) . 2_656 ?
O2 B1 Rb2 154.3(7) . . ?
O2 B1 Rb2 125.1(6) . 2_545 ?
O2 B1 O1 120.8(9) . . ?
O2 B1 O3 122.9(9) . . ?
O3 B1 K3 86.7(6) . . ?
O3 B1 Rb1 107.4(6) . 2_656 ?
O3 B1 Rb2 94.3(6) . 2_545 ?
O3 B1 Rb2 72.7(5) . . ?
K3 B2 K3 88.1(2) 1_565 2_655 ?
K3 B2 Rb2 100.9(3) 2_655 1_655 ?
K3 B2 Rb2 60.43(18) 1_565 1_655 ?
K3 B2 Rb2 63.99(19) 2_655 2_645 ?
K3 B2 Rb2 115.4(3) 1_565 2_645 ?
Rb2 B2 Rb2 69.2(2) 2_645 1_655 ?
O3 B2 K3 89.7(5) . 1_565 ?
O3 B2 K3 51.8(4) . 2_655 ?
O3 B2 Rb2 142.0(6) . 1_655 ?
O3 B2 Rb2 109.6(5) . 2_645 ?
O3 B2 F1 101.5(7) . . ?
O4 B2 K3 106.5(5) . 2_655 ?
O4 B2 K3 154.9(6) . 1_565 ?
O4 B2 Rb2 57.4(5) . 2_645 ?
O4 B2 Rb2 96.2(5) . 1_655 ?
O4 B2 O3 115.4(8) . . ?
O4 B2 O5 114.8(8) . . ?
O4 B2 F1 109.6(8) . . ?
O5 B2 K3 138.6(6) . 2_655 ?
O5 B2 K3 52.5(4) . 1_565 ?
O5 B2 Rb2 72.6(5) . 1_655 ?
O5 B2 Rb2 139.3(6) . 2_645 ?
O5 B2 O3 109.0(8) . . ?
O5 B2 F1 105.3(8) . . ?
F1 B2 K3 61.7(4) . 1_565 ?
F1 B2 K3 55.7(4) . 2_655 ?
F1 B2 Rb2 54.4(4) . 2_645 ?
F1 B2 Rb2 45.3(4) . 1_655 ?
K3 B3 Rb1 155.4(3) . 2_756 ?
Rb2 B3 K3 72.11(19) 2_645 . ?
Rb2 B3 Rb1 131.9(3) 2_645 2_756 ?
O1 B3 K3 129.5(6) 1_655 . ?
O1 B3 Rb1 73.3(4) 1_655 2_756 ?
O1 B3 Rb2 58.8(4) 1_655 2_645 ?
O4 B3 K3 43.5(4) . . ?
O4 B3 Rb1 147.7(6) . 2_756 ?
O4 B3 Rb2 57.6(4) . 2_645 ?
O4 B3 O1 108.9(7) . 1_655 ?
O4 B3 O6 110.1(7) . . ?
O4 B3 O8 110.5(7) . 2_746 ?
O6 B3 K3 120.1(6) . . ?
O6 B3 Rb1 43.7(4) . 2_756 ?
O6 B3 Rb2 149.6(6) . 2_645 ?
O6 B3 O1 108.6(8) . 1_655 ?
O8 B3 K3 67.3(4) 2_746 . ?
O8 B3 Rb1 98.1(5) 2_746 2_756 ?
O8 B3 Rb2 101.6(5) 2_746 2_645 ?
O8 B3 O1 110.0(7) 2_746 1_655 ?
O8 B3 O6 108.8(7) 2_746 . ?
Rb1 B4 Rb1 76.2(2) . 2_656 ?
Rb1 B4 Rb1 96.2(3) 2_756 . ?
Rb1 B4 Rb1 141.7(3) 2_756 2_656 ?
O5 B4 Rb1 136.7(7) . 2_756 ?
O5 B4 Rb1 113.9(6) . . ?
O5 B4 Rb1 78.1(5) . 2_656 ?
O6 B4 Rb1 58.6(5) . . ?
O6 B4 Rb1 51.8(4) . 2_756 ?
O6 B4 Rb1 134.8(7) . 2_656 ?
O6 B4 O5 119.2(9) . . ?
O7 B4 Rb1 87.6(5) . 2_756 ?
O7 B4 Rb1 57.3(5) . 2_656 ?
O7 B4 Rb1 98.0(6) . . ?
O7 B4 O5 116.3(9) . . ?
O7 B4 O6 124.5(9) . . ?
K3 B5 Rb1 61.39(18) 2_656 2_656 ?
K3 B5 Rb1 155.4(4) 2_656 2_756 ?
K3 B5 Rb1 113.8(3) 2_656 1_565 ?
Rb1 B5 Rb1 134.6(3) 2_656 2_756 ?
Rb1 B5 Rb1 90.1(2) 1_565 2_756 ?
Rb1 B5 Rb1 76.9(2) 2_656 1_565 ?
Rb2 B5 K3 63.61(19) 2_646 2_656 ?
Rb2 B5 Rb1 118.0(3) 2_646 2_656 ?
Rb2 B5 Rb1 92.3(3) 2_646 2_756 ?
Rb2 B5 Rb1 154.0(3) 2_646 1_565 ?
O2 B5 K3 50.3(4) 2_656 2_656 ?
O2 B5 Rb1 65.0(5) 2_656 2_656 ?
O2 B5 Rb1 66.6(5) 2_656 1_565 ?
O2 B5 Rb1 146.8(6) 2_656 2_756 ?
O2 B5 Rb2 99.0(6) 2_656 2_646 ?
O7 B5 K3 124.1(6) . 2_656 ?
O7 B5 Rb1 62.7(4) . 2_656 ?
O7 B5 Rb1 52.2(4) . 1_565 ?
O7 B5 Rb1 74.9(5) . 2_756 ?
O7 B5 Rb2 152.6(7) . 2_646 ?
O7 B5 O2 104.9(8) . 2_656 ?
O8 B5 K3 117.1(6) . 2_656 ?
O8 B5 Rb1 177.5(7) . 2_656 ?
O8 B5 Rb1 102.4(6) . 1_565 ?
O8 B5 Rb1 47.6(4) . 2_756 ?
O8 B5 Rb2 61.8(5) . 2_646 ?
O8 B5 O2 112.4(8) . 2_656 ?
O8 B5 O7 118.8(8) . . ?
O8 B5 F2 107.4(8) . . ?
F2 B5 K3 55.3(4) . 2_656 ?
F2 B5 Rb1 73.6(5) . 2_656 ?
F2 B5 Rb1 150.0(6) . 1_565 ?
F2 B5 Rb1 106.7(6) . 2_756 ?
F2 B5 Rb2 52.3(4) . 2_646 ?
F2 B5 O2 104.9(8) . 2_656 ?
F2 B5 O7 107.5(8) . . ?
Rb2 O1 Rb1 87.79(16) . 2_656 ?
Rb2 O1 Rb1 175.6(2) 2_545 2_656 ?
Rb2 O1 Rb2 88.93(18) . 2_545 ?
B1 O1 Rb1 71.6(5) . 2_656 ?
B1 O1 Rb2 110.5(5) . . ?
B1 O1 Rb2 112.4(5) . 2_545 ?
B1 O1 B3 119.9(7) . 1_455 ?
B3 O1 Rb1 83.3(5) 1_455 2_656 ?
B3 O1 Rb2 122.3(5) 1_455 . ?
B3 O1 Rb2 96.0(5) 1_455 2_545 ?
K3 O2 Rb1 153.9(2) . 2_656 ?
K3 O2 Rb1 73.25(16) . . ?
Rb1 O2 Rb1 85.91(16) . 2_656 ?
B1 O2 K3 106.4(6) . . ?
B1 O2 Rb1 145.1(6) . . ?
B1 O2 Rb1 81.8(5) . 2_656 ?
B1 O2 B5 122.4(8) . 2_646 ?
B5 O2 K3 105.5(5) 2_646 . ?
B5 O2 Rb1 89.6(5) 2_646 2_656 ?
B5 O2 Rb1 89.8(5) 2_646 . ?
K3 O3 Rb2 85.06(16) 2_655 . ?
B1 O3 K3 123.1(6) . 2_655 ?
B1 O3 Rb2 84.3(5) . . ?
B1 O3 B2 126.4(8) . . ?
B2 O3 K3 103.2(5) . 2_655 ?
B2 O3 Rb2 128.5(5) . . ?
K3 O4 Rb1 66.49(14) . . ?
K3 O4 Rb2 93.86(19) . 2_645 ?
Rb2 O4 Rb1 147.9(2) 2_645 . ?
B2 O4 K3 121.7(5) . . ?
B2 O4 Rb1 112.6(5) . . ?
B2 O4 Rb2 99.2(5) . 2_645 ?
B2 O4 B3 118.9(7) . . ?
B3 O4 K3 114.9(5) . . ?
B3 O4 Rb1 70.5(5) . . ?
B3 O4 Rb2 98.1(5) . 2_645 ?
K3 O5 Rb1 101.38(19) 1_565 2_656 ?
K3 O5 Rb2 67.87(16) 1_565 1_655 ?
Rb2 O5 Rb1 161.7(2) 1_655 2_656 ?
B2 O5 K3 102.5(5) . 1_565 ?
B2 O5 Rb1 113.5(6) . 2_656 ?
B2 O5 Rb2 83.9(5) . 1_655 ?
B4 O5 K3 133.5(6) . 1_565 ?
B4 O5 Rb1 79.7(5) . 2_656 ?
B4 O5 Rb2 96.9(5) . 1_655 ?
B4 O5 B2 119.8(8) . . ?
Rb1 O6 Rb1 124.0(2) 2_756 . ?
B3 O6 Rb1 115.5(5) . 2_756 ?
B3 O6 Rb1 88.9(5) . . ?
B4 O6 Rb1 106.5(5) . 2_756 ?
B4 O6 Rb1 99.7(6) . . ?
B4 O6 B3 121.7(7) . . ?
Rb1 O7 Rb1 93.69(18) 1_565 2_656 ?
B4 O7 Rb1 118.3(6) . 1_565 ?
B4 O7 Rb1 101.3(5) . 2_656 ?
B4 O7 B5 133.1(8) . . ?
B5 O7 Rb1 92.4(5) . 2_656 ?
B5 O7 Rb1 105.2(5) . 1_565 ?
Rb1 O8 K3 68.20(13) 2_756 2_756 ?
Rb1 O8 Rb2 119.2(2) 2_756 2_646 ?
Rb2 O8 K3 68.04(13) 2_646 2_756 ?
B3 O8 K3 88.4(4) 2_756 2_756 ?
B3 O8 Rb1 92.6(5) 2_756 2_756 ?
B3 O8 Rb2 125.8(5) 2_756 2_646 ?
B5 O8 K3 156.3(6) . 2_756 ?
B5 O8 Rb1 111.8(5) . 2_756 ?
B5 O8 Rb2 93.7(5) . 2_646 ?
B5 O8 B3 115.0(7) . 2_756 ?
K3 F1 K3 108.30(17) 2_655 1_565 ?
K3 F1 Rb2 79.23(15) 2_655 2_645 ?
Rb2 F1 K3 148.7(2) 1_655 2_655 ?
Rb2 F1 K3 164.1(2) 2_645 1_565 ?
Rb2 F1 K3 75.54(14) 1_655 1_565 ?
Rb2 F1 Rb2 90.75(15) 1_655 2_645 ?
B2 F1 K3 92.1(5) . 1_565 ?
B2 F1 K3 98.5(5) . 2_655 ?
B2 F1 Rb2 112.6(5) . 1_655 ?
B2 F1 Rb2 100.8(5) . 2_645 ?
K3 F2 Rb1 68.44(12) 2_656 2_656 ?
Rb1 F2 K3 119.20(19) . 2_656 ?
Rb1 F2 Rb1 91.44(15) . 2_656 ?
Rb2 F2 K3 79.43(15) 2_646 2_656 ?
Rb2 F2 Rb1 147.9(2) 2_646 2_656 ?
Rb2 F2 Rb1 105.67(18) 2_646 . ?
B5 F2 K3 100.3(5) . 2_656 ?
B5 F2 Rb1 134.2(5) . . ?
B5 F2 Rb1 81.9(5) . 2_656 ?
B5 F2 Rb2 103.4(5) . 2_646 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
K3 B1 O1 Rb1 135.7(9) . . . 2_656 ?
K3 B1 O1 Rb2 -144.0(7) . . . . ?
K3 B1 O1 Rb2 -46.4(10) . . . 2_545 ?
K3 B1 O1 B3 65.2(12) . . . 1_455 ?
K3 B1 O2 Rb1 84.1(9) . . . . ?
K3 B1 O2 Rb1 154.6(3) . . . 2_656 ?
K3 B1 O2 B5 -121.2(9) . . . 2_646 ?
K3 B1 O3 K3 83.6(5) . . . 2_655 ?
K3 B1 O3 Rb2 163.9(2) . . . . ?
K3 B1 O3 B2 -61.3(9) . . . . ?
K3 B2 O3 K3 87.8(3) 1_565 . . 2_655 ?
K3 B2 O3 Rb2 -6.4(6) 1_565 . . . ?
K3 B2 O3 Rb2 -94.2(5) 2_655 . . . ?
K3 B2 O3 B1 150.3(10) 2_655 . . . ?
K3 B2 O3 B1 -121.9(8) 1_565 . . . ?
K3 B2 O4 K3 -57.5(6) 2_655 . . . ?
K3 B2 O4 K3 179.1(11) 1_565 . . . ?
K3 B2 O4 Rb1 -133.0(3) 2_655 . . . ?
K3 B2 O4 Rb1 103.6(14) 1_565 . . . ?
K3 B2 O4 Rb2 -80.5(15) 1_565 . . 2_645 ?
K3 B2 O4 Rb2 42.9(4) 2_655 . . 2_645 ?
K3 B2 O4 B3 24.2(19) 1_565 . . . ?
K3 B2 O4 B3 147.6(6) 2_655 . . . ?
K3 B2 O5 K3 -21.1(10) 2_655 . . 1_565 ?
K3 B2 O5 Rb1 87.4(9) 2_655 . . 2_656 ?
K3 B2 O5 Rb1 108.4(4) 1_565 . . 2_656 ?
K3 B2 O5 Rb2 -86.8(8) 2_655 . . 1_655 ?
K3 B2 O5 Rb2 -65.7(2) 1_565 . . 1_655 ?
K3 B2 O5 B4 -160.1(10) 1_565 . . . ?
K3 B2 O5 B4 178.8(7) 2_655 . . . ?
K3 B2 F1 K3 -108.9(2) 1_565 . . 2_655 ?
K3 B2 F1 K3 108.9(2) 2_655 . . 1_565 ?
K3 B2 F1 Rb2 -80.6(2) 2_655 . . 2_645 ?
K3 B2 F1 Rb2 170.6(3) 1_565 . . 2_645 ?
K3 B2 F1 Rb2 75.2(3) 1_565 . . 1_655 ?
K3 B2 F1 Rb2 -175.9(4) 2_655 . . 1_655 ?
K3 B3 O4 Rb1 50.9(4) . . . . ?
K3 B3 O4 Rb2 -98.1(4) . . . 2_645 ?
K3 B3 O4 B2 156.6(9) . . . . ?
K3 B3 O6 Rb1 28.5(5) . . . . ?
K3 B3 O6 Rb1 156.1(3) . . . 2_756 ?
K3 B3 O6 B4 -72.2(10) . . . . ?
K3 B5 O7 Rb1 0.7(6) 2_656 . . 2_656 ?
K3 B5 O7 Rb1 95.2(6) 2_656 . . 1_565 ?
K3 B5 O7 B4 -107.1(10) 2_656 . . . ?
K3 B5 O8 K3 71.0(15) 2_656 . . 2_756 ?
K3 B5 O8 Rb1 156.3(3) 2_656 . . 2_756 ?
K3 B5 O8 Rb2 32.7(5) 2_656 . . 2_646 ?
K3 B5 O8 B3 -99.8(8) 2_656 . . 2_756 ?
K3 B5 F2 Rb1 150.3(7) 2_656 . . . ?
K3 B5 F2 Rb1 66.21(19) 2_656 . . 2_656 ?
K3 B5 F2 Rb2 -81.5(3) 2_656 . . 2_646 ?
Rb1 B1 O1 Rb2 177.9(3) 2_656 . . 2_545 ?
Rb1 B1 O1 Rb2 80.3(3) 2_656 . . . ?
Rb1 B1 O1 B3 -70.5(7) 2_656 . . 1_455 ?
Rb1 B1 O2 K3 -154.6(3) 2_656 . . . ?
Rb1 B1 O2 Rb1 -70.5(9) 2_656 . . . ?
Rb1 B1 O2 B5 84.2(8) 2_656 . . 2_646 ?
Rb1 B1 O3 K3 -153.9(3) 2_656 . . 2_655 ?
Rb1 B1 O3 Rb2 -73.5(3) 2_656 . . . ?
Rb1 B1 O3 B2 61.2(10) 2_656 . . . ?
Rb1 B3 O4 K3 -143.5(8) 2_756 . . . ?
Rb1 B3 O4 Rb1 -92.6(10) 2_756 . . . ?
Rb1 B3 O4 Rb2 118.4(10) 2_756 . . 2_645 ?
Rb1 B3 O4 B2 13.1(15) 2_756 . . . ?
Rb1 B3 O6 Rb1 -127.6(4) 2_756 . . . ?
Rb1 B3 O6 B4 131.7(10) 2_756 . . . ?
Rb1 B4 O5 K3 -65.1(12) 2_756 . . 1_565 ?
Rb1 B4 O5 K3 96.0(7) 2_656 . . 1_565 ?
Rb1 B4 O5 K3 164.9(4) . . . 1_565 ?
Rb1 B4 O5 Rb1 69.0(4) . . . 2_656 ?
Rb1 B4 O5 Rb1 -161.1(9) 2_756 . . 2_656 ?
Rb1 B4 O5 Rb2 0.7(9) 2_756 . . 1_655 ?
Rb1 B4 O5 Rb2 161.83(18) 2_656 . . 1_655 ?
Rb1 B4 O5 Rb2 -129.2(4) . . . 1_655 ?
Rb1 B4 O5 B2 -111.2(8) 2_656 . . . ?
Rb1 B4 O5 B2 -42.3(10) . . . . ?
Rb1 B4 O5 B2 87.7(11) 2_756 . . . ?
Rb1 B4 O6 Rb1 1.2(9) 2_656 . . . ?
Rb1 B4 O6 Rb1 130.0(4) 2_756 . . . ?
Rb1 B4 O6 Rb1 -128.8(6) 2_656 . . 2_756 ?
Rb1 B4 O6 Rb1 -130.0(4) . . . 2_756 ?
Rb1 B4 O6 B3 -135.3(9) 2_756 . . . ?
Rb1 B4 O6 B3 95.9(10) 2_656 . . . ?
Rb1 B4 O6 B3 94.7(8) . . . . ?
Rb1 B4 O7 Rb1 95.7(4) 2_756 . . 1_565 ?
Rb1 B4 O7 Rb1 -100.5(5) 2_656 . . 1_565 ?
Rb1 B4 O7 Rb1 -163.8(2) 2_756 . . 2_656 ?
Rb1 B4 O7 Rb1 -168.4(3) . . . 1_565 ?
Rb1 B4 O7 Rb1 -67.9(3) . . . 2_656 ?
Rb1 B4 O7 B5 -59.7(10) 2_756 . . . ?
Rb1 B4 O7 B5 36.3(11) . . . . ?
Rb1 B4 O7 B5 104.2(10) 2_656 . . . ?
Rb1 B5 O7 Rb1 94.5(3) 2_656 . . 1_565 ?
Rb1 B5 O7 Rb1 -94.5(3) 1_565 . . 2_656 ?
Rb1 B5 O7 Rb1 -102.2(3) 2_756 . . 1_565 ?
Rb1 B5 O7 Rb1 163.32(19) 2_756 . . 2_656 ?
Rb1 B5 O7 B4 -107.9(10) 2_656 . . . ?
Rb1 B5 O7 B4 157.6(11) 1_565 . . . ?
Rb1 B5 O7 B4 55.4(9) 2_756 . . . ?
Rb1 B5 O8 K3 -85.3(14) 2_756 . . 2_756 ?
Rb1 B5 O8 K3 -163.8(11) 1_565 . . 2_756 ?
Rb1 B5 O8 Rb1 -78.6(4) 1_565 . . 2_756 ?
Rb1 B5 O8 Rb2 -123.5(4) 2_756 . . 2_646 ?
Rb1 B5 O8 Rb2 157.9(2) 1_565 . . 2_646 ?
Rb1 B5 O8 B3 25.3(8) 1_565 . . 2_756 ?
Rb1 B5 O8 B3 103.9(8) 2_756 . . 2_756 ?
Rb1 B5 F2 K3 -77.4(12) 1_565 . . 2_656 ?
Rb1 B5 F2 K3 -66.21(19) 2_656 . . 2_656 ?
Rb1 B5 F2 K3 161.2(2) 2_756 . . 2_656 ?
Rb1 B5 F2 Rb1 84.1(6) 2_656 . . . ?
Rb1 B5 F2 Rb1 -48.5(8) 2_756 . . . ?
Rb1 B5 F2 Rb1 -11.2(11) 1_565 . . 2_656 ?
Rb1 B5 F2 Rb1 72.9(14) 1_565 . . . ?
Rb1 B5 F2 Rb1 -132.5(3) 2_756 . . 2_656 ?
Rb1 B5 F2 Rb2 -147.7(2) 2_656 . . 2_646 ?
Rb1 B5 F2 Rb2 79.8(4) 2_756 . . 2_646 ?
Rb1 B5 F2 Rb2 -158.9(10) 1_565 . . 2_646 ?
Rb2 B1 O1 Rb1 -80.3(3) . . . 2_656 ?
Rb2 B1 O1 Rb1 -177.9(3) 2_545 . . 2_656 ?
Rb2 B1 O1 Rb2 -97.6(5) 2_545 . . . ?
Rb2 B1 O1 Rb2 97.6(5) . . . 2_545 ?
Rb2 B1 O1 B3 -150.9(9) . . . 1_455 ?
Rb2 B1 O1 B3 111.5(8) 2_545 . . 1_455 ?
Rb2 B1 O2 K3 71.4(7) 2_545 . . . ?
Rb2 B1 O2 K3 -174.9(12) . . . . ?
Rb2 B1 O2 Rb1 -20.3(14) . . . 2_656 ?
Rb2 B1 O2 Rb1 -134.0(6) 2_545 . . 2_656 ?
Rb2 B1 O2 Rb1 155.5(5) 2_545 . . . ?
Rb2 B1 O2 Rb1 -90.9(17) . . . . ?
Rb2 B1 O2 B5 -49.8(11) 2_545 . . 2_646 ?
Rb2 B1 O2 B5 63.9(17) . . . 2_646 ?
Rb2 B1 O3 K3 -15.1(6) 2_545 . . 2_655 ?
Rb2 B1 O3 K3 -80.3(5) . . . 2_655 ?
Rb2 B1 O3 Rb2 65.3(2) 2_545 . . . ?
Rb2 B1 O3 B2 -160.0(8) 2_545 . . . ?
Rb2 B1 O3 B2 134.8(9) . . . . ?
Rb2 B2 O3 K3 -29.2(5) 2_645 . . 2_655 ?
Rb2 B2 O3 K3 51.8(10) 1_655 . . 2_655 ?
Rb2 B2 O3 Rb2 -42.4(12) 1_655 . . . ?
Rb2 B2 O3 Rb2 -123.4(4) 2_645 . . . ?
Rb2 B2 O3 B1 -157.9(8) 1_655 . . . ?
Rb2 B2 O3 B1 121.1(8) 2_645 . . . ?
Rb2 B2 O4 K3 -160.8(3) 1_655 . . . ?
Rb2 B2 O4 K3 -100.4(5) 2_645 . . . ?
Rb2 B2 O4 Rb1 -175.9(4) 2_645 . . . ?
Rb2 B2 O4 Rb1 123.7(3) 1_655 . . . ?
Rb2 B2 O4 Rb2 -60.4(3) 1_655 . . 2_645 ?
Rb2 B2 O4 B3 104.7(7) 2_645 . . . ?
Rb2 B2 O4 B3 44.3(8) 1_655 . . . ?
Rb2 B2 O5 K3 65.7(2) 1_655 . . 1_565 ?
Rb2 B2 O5 K3 86.5(8) 2_645 . . 1_565 ?
Rb2 B2 O5 Rb1 174.1(3) 1_655 . . 2_656 ?
Rb2 B2 O5 Rb1 -165.1(6) 2_645 . . 2_656 ?
Rb2 B2 O5 Rb2 20.8(8) 2_645 . . 1_655 ?
Rb2 B2 O5 B4 -94.4(8) 1_655 . . . ?
Rb2 B2 O5 B4 -73.7(12) 2_645 . . . ?
Rb2 B2 F1 K3 -75.2(3) 1_655 . . 1_565 ?
Rb2 B2 F1 K3 175.9(4) 1_655 . . 2_655 ?
Rb2 B2 F1 K3 -170.6(3) 2_645 . . 1_565 ?
Rb2 B2 F1 K3 80.6(2) 2_645 . . 2_655 ?
Rb2 B2 F1 Rb2 95.4(3) 1_655 . . 2_645 ?
Rb2 B2 F1 Rb2 -95.4(3) 2_645 . . 1_655 ?
Rb2 B3 O4 K3 98.1(4) 2_645 . . . ?
Rb2 B3 O4 Rb1 149.0(2) 2_645 . . . ?
Rb2 B3 O4 B2 -105.3(8) 2_645 . . . ?
Rb2 B3 O6 Rb1 135.2(10) 2_645 . . . ?
Rb2 B3 O6 Rb1 -97.2(10) 2_645 . . 2_756 ?
Rb2 B3 O6 B4 34.5(16) 2_645 . . . ?
Rb2 B5 O7 Rb1 -166.8(11) 2_646 . . 1_565 ?
Rb2 B5 O7 Rb1 98.7(13) 2_646 . . 2_656 ?
Rb2 B5 O7 B4 -9(2) 2_646 . . . ?
Rb2 B5 O8 K3 38.3(13) 2_646 . . 2_756 ?
Rb2 B5 O8 Rb1 123.5(4) 2_646 . . 2_756 ?
Rb2 B5 O8 B3 -132.6(7) 2_646 . . 2_756 ?
Rb2 B5 F2 K3 81.5(3) 2_646 . . 2_656 ?
Rb2 B5 F2 Rb1 -128.2(7) 2_646 . . . ?
Rb2 B5 F2 Rb1 147.7(2) 2_646 . . 2_656 ?
O1 B1 O2 K3 129.0(8) . . . . ?
O1 B1 O2 Rb1 -147.0(7) . . . . ?
O1 B1 O2 Rb1 -76.4(8) . . . 2_656 ?
O1 B1 O2 B5 7.8(13) . . . 2_646 ?
O1 B1 O3 K3 -59.6(10) . . . 2_655 ?
O1 B1 O3 Rb2 20.8(8) . . . . ?
O1 B1 O3 B2 155.6(8) . . . . ?
O1 B3 O4 K3 128.1(6) 1_655 . . . ?
O1 B3 O4 Rb1 179.0(8) 1_655 . . . ?
O1 B3 O4 Rb2 30.0(7) 1_655 . . 2_645 ?
O1 B3 O4 B2 -75.4(10) 1_655 . . . ?
O1 B3 O6 Rb1 -165.4(6) 1_655 . . . ?
O1 B3 O6 Rb1 -37.8(8) 1_655 . . 2_756 ?
O1 B3 O6 B4 93.9(9) 1_655 . . . ?
O2 B1 O1 Rb1 70.7(8) . . . 2_656 ?
O2 B1 O1 Rb2 151.0(7) . . . . ?
O2 B1 O1 Rb2 -111.4(8) . . . 2_545 ?
O2 B1 O1 B3 0.2(13) . . . 1_455 ?
O2 B1 O3 K3 122.3(8) . . . 2_655 ?
O2 B1 O3 Rb2 -157.3(9) . . . . ?
O2 B1 O3 B2 -22.6(15) . . . . ?
O2 B5 O7 Rb1 43.4(7) 2_656 . . 1_565 ?
O2 B5 O7 Rb1 -51.1(7) 2_656 . . 2_656 ?
O2 B5 O7 B4 -158.9(9) 2_656 . . . ?
O2 B5 O8 K3 126.6(12) 2_656 . . 2_756 ?
O2 B5 O8 Rb1 -148.2(6) 2_656 . . 2_756 ?
O2 B5 O8 Rb2 88.3(7) 2_656 . . 2_646 ?
O2 B5 O8 B3 -44.3(11) 2_656 . . 2_756 ?
O2 B5 F2 K3 -8.4(7) 2_656 . . 2_656 ?
O2 B5 F2 Rb1 141.8(5) 2_656 . . . ?
O2 B5 F2 Rb1 57.8(6) 2_656 . . 2_656 ?
O2 B5 F2 Rb2 -89.9(6) 2_656 . . 2_646 ?
O3 B1 O1 Rb1 -107.5(8) . . . 2_656 ?
O3 B1 O1 Rb2 70.5(9) . . . 2_545 ?
O3 B1 O1 Rb2 -27.1(10) . . . . ?
O3 B1 O1 B3 -178.0(8) . . . 1_455 ?
O3 B1 O2 K3 -53.0(10) . . . . ?
O3 B1 O2 Rb1 101.6(9) . . . 2_656 ?
O3 B1 O2 Rb1 31.1(16) . . . . ?
O3 B1 O2 B5 -174.2(9) . . . 2_646 ?
O3 B2 O4 K3 -2.5(11) . . . . ?
O3 B2 O4 Rb1 -78.0(8) . . . . ?
O3 B2 O4 Rb2 97.9(7) . . . 2_645 ?
O3 B2 O4 B3 -157.4(8) . . . . ?
O3 B2 O5 K3 -74.3(7) . . . 1_565 ?
O3 B2 O5 Rb1 34.2(8) . . . 2_656 ?
O3 B2 O5 Rb2 -140.0(7) . . . 1_655 ?
O3 B2 O5 B4 125.6(9) . . . . ?
O3 B2 F1 K3 -25.5(7) . . . 2_655 ?
O3 B2 F1 K3 83.4(6) . . . 1_565 ?
O3 B2 F1 Rb2 -106.0(6) . . . 2_645 ?
O3 B2 F1 Rb2 158.6(5) . . . 1_655 ?
O4 B2 O3 K3 -91.5(8) . . . 2_655 ?
O4 B2 O3 Rb2 174.3(5) . . . . ?
O4 B2 O3 B1 58.8(12) . . . . ?
O4 B2 O5 K3 154.5(7) . . . 1_565 ?
O4 B2 O5 Rb1 -97.0(8) . . . 2_656 ?
O4 B2 O5 Rb2 88.8(8) . . . 1_655 ?
O4 B2 O5 B4 -5.6(13) . . . . ?
O4 B2 F1 K3 -154.2(6) . . . 1_565 ?
O4 B2 F1 K3 97.0(6) . . . 2_655 ?
O4 B2 F1 Rb2 -78.9(7) . . . 1_655 ?
O4 B2 F1 Rb2 16.4(7) . . . 2_645 ?
O4 B3 O6 Rb1 -156.9(5) . . . 2_756 ?
O4 B3 O6 Rb1 75.5(7) . . . . ?
O4 B3 O6 B4 -25.2(12) . . . . ?
O5 B2 O3 K3 137.6(6) . . . 2_655 ?
O5 B2 O3 Rb2 43.4(10) . . . . ?
O5 B2 O3 B1 -72.1(12) . . . . ?
O5 B2 O4 K3 125.5(7) . . . . ?
O5 B2 O4 Rb1 50.1(9) . . . . ?
O5 B2 O4 Rb2 -134.1(7) . . . 2_645 ?
O5 B2 O4 B3 -29.4(12) . . . . ?
O5 B2 F1 K3 -30.2(6) . . . 1_565 ?
O5 B2 F1 K3 -139.0(6) . . . 2_655 ?
O5 B2 F1 Rb2 45.1(8) . . . 1_655 ?
O5 B2 F1 Rb2 140.4(6) . . . 2_645 ?
O5 B4 O6 Rb1 -101.7(8) . . . . ?
O5 B4 O6 Rb1 128.3(8) . . . 2_756 ?
O5 B4 O6 B3 -7.0(14) . . . . ?
O5 B4 O7 Rb1 -46.6(10) . . . 1_565 ?
O5 B4 O7 Rb1 53.9(9) . . . 2_656 ?
O5 B4 O7 B5 158.0(9) . . . . ?
O6 B3 O4 K3 -113.0(7) . . . . ?
O6 B3 O4 Rb1 -62.1(6) . . . . ?
O6 B3 O4 Rb2 148.9(6) . . . 2_645 ?
O6 B3 O4 B2 43.6(11) . . . . ?
O6 B4 O5 K3 -129.0(8) . . . 1_565 ?
O6 B4 O5 Rb1 135.0(9) . . . 2_656 ?
O6 B4 O5 Rb2 -63.1(9) . . . 1_655 ?
O6 B4 O5 B2 23.8(14) . . . . ?
O6 B4 O7 Rb1 -125.1(9) . . . 2_656 ?
O6 B4 O7 Rb1 134.4(8) . . . 1_565 ?
O6 B4 O7 B5 -20.9(16) . . . . ?
O7 B4 O5 K3 52.0(12) . . . 1_565 ?
O7 B4 O5 Rb1 -44.0(7) . . . 2_656 ?
O7 B4 O5 Rb2 117.8(8) . . . 1_655 ?
O7 B4 O5 B2 -155.2(8) . . . . ?
O7 B4 O6 Rb1 -52.7(10) . . . 2_756 ?
O7 B4 O6 Rb1 77.2(9) . . . . ?
O7 B4 O6 B3 171.9(9) . . . . ?
O7 B5 O8 K3 -110.5(14) . . . 2_756 ?
O7 B5 O8 Rb1 -25.2(10) . . . 2_756 ?
O7 B5 O8 Rb2 -148.7(8) . . . 2_646 ?
O7 B5 O8 B3 78.7(11) . . . 2_756 ?
O7 B5 F2 K3 -119.7(6) . . . 2_656 ?
O7 B5 F2 Rb1 -53.5(6) . . . 2_656 ?
O7 B5 F2 Rb1 30.5(11) . . . . ?
O7 B5 F2 Rb2 158.8(6) . . . 2_646 ?
O8 B3 O4 K3 7.2(9) 2_746 . . . ?
O8 B3 O4 Rb1 58.1(6) 2_746 . . . ?
O8 B3 O4 Rb2 -90.9(7) 2_746 . . 2_645 ?
O8 B3 O4 B2 163.8(8) 2_746 . . . ?
O8 B3 O6 Rb1 81.9(7) 2_746 . . 2_756 ?
O8 B3 O6 Rb1 -45.7(6) 2_746 . . . ?
O8 B3 O6 B4 -146.4(8) 2_746 . . . ?
O8 B5 O7 Rb1 -177.7(8) . . . 2_656 ?
O8 B5 O7 Rb1 -83.2(9) . . . 1_565 ?
O8 B5 O7 B4 74.4(14) . . . . ?
O8 B5 F2 K3 111.3(6) . . . 2_656 ?
O8 B5 F2 Rb1 177.5(7) . . . 2_656 ?
O8 B5 F2 Rb1 -98.4(8) . . . . ?
O8 B5 F2 Rb2 29.8(8) . . . 2_646 ?
F1 B2 O3 K3 26.9(7) . . . 2_655 ?
F1 B2 O3 Rb2 -67.3(8) . . . . ?
F1 B2 O3 B1 177.2(8) . . . . ?
F1 B2 O4 K3 -116.2(6) . . . . ?
F1 B2 O4 Rb1 168.3(5) . . . . ?
F1 B2 O4 Rb2 -15.8(7) . . . 2_645 ?
F1 B2 O4 B3 88.9(9) . . . . ?
F1 B2 O5 K3 33.9(7) . . . 1_565 ?
F1 B2 O5 Rb1 142.3(5) . . . 2_656 ?
F1 B2 O5 Rb2 -31.8(6) . . . 1_655 ?
F1 B2 O5 B4 -126.3(9) . . . . ?
F2 B5 O7 Rb1 60.2(7) . . . 2_656 ?
F2 B5 O7 Rb1 154.7(6) . . . 1_565 ?
F2 B5 O7 B4 -47.6(13) . . . . ?
F2 B5 O8 K3 11.7(19) . . . 2_756 ?
F2 B5 O8 Rb1 97.0(7) . . . 2_756 ?
F2 B5 O8 Rb2 -26.6(7) . . . 2_646 ?
F2 B5 O8 B3 -159.1(7) . . . 2_756 ?

_olex2_submission_special_instructions 'No special instructions were received'
